In polymerization kinetic, *steady state conditions* must obtain, i.e. where the rate of generation of free radicals (initiation) is equal to the rate at which they disappear (termination). This implies a constant overall concentration of propagating free radicals, [*M* ]. The equation for the steady state conditions is:

$$R\_i = R\_t = -\frac{d[R\bullet]}{dt} = 2k\_t[M\bullet]^2\tag{16}$$

In practice, most free-radical polymerizations operate under steady state conditions after an induction period wich may be at most a few seconds. When Equation 2.16 is rearranged,

$$\mathbb{E}\left[M\bullet\right] = \left(\frac{R\_i}{2k\_t}\right)^{\bigvee\_2} \tag{17}$$

and a general expression for the rate of polymerization can be obtained by combining Equation 2.12 and 2.17,

$$R\_p = k\_p [M] \left(\frac{R\_i}{2k\_t}\right)^{\frac{1}{2}} \tag{18}$$

Emulsion Polymerization:

Effects of Polymerization Variables on the Properties of Vinyl Acetate Based Emulsion Polymers 47

micelles. These micelles are the principal locus for the initiation of polymer particle nuclei. In other words, they act as a meeting place for the hydrophobic monomer and the watersoluble initiator. Since they exhibit an extremely large oil-water interfacial area for diffusing of free-radicals and have high monomer concentration. On the other hand, a small amount of particle initiation can occur within the continuous aqueous phase. Monomer molecules dissolved in this phase are first polymerized by waterborne free-radicals. This would result in the increased hdrophobicity of oligomeric radicals. When a critical chain length is achieved, these oligomeric radicals become so hydrophobic that they show a strong tendency to enter the monomer-swollen micelles and then continue to propagate by reacting with those monomer molecules. But this nucleation becomes less significant as the amount of micellar emulsifier in the system increases. The amount of polymerization occurring in the monomer droplets is regarded as being a very minor proportion of the whole because of their small surface area for diffusing of the free-radicals. As a result, monomer-swollen micelles are favored as the sites of the nucleation of polymer particles. Therefore, this nucleation mechanism, proposed by Harkins and Smith and Ewart and modified by

After nucleation, monomer-swollen micelles are transformed into polymer particles swollen with monomer. The monomers are then acquired to the particles continuously from monomer droplets by diffusion through the aqueous phase, because monomer has been consumed with in the reaction loci by the polymerization process. Thus, the micelles grow from tiny groups of emulsifier and monomer molecules to larger groups of polymer molecules held in emulsion by the action of the emulsifier molecules located on the exterior surfaces of the particles. This action of the emulsifiers for providing colloidal stability of the growing particle nuclei occurs by emulsifiers supplied from the aqueous phase; this in turn tends to leads to dissociation of micelles containing monomer in which polymerization has not yet started. With the continued adsorption of micellar emulsifiers on to growing particles, the micelles start to disappear (Figure 1.b). The particle nucleation stage (Interval I) ends with this disappearance of the micelles at relatively early in the reaction (e.g. between 10% and 20% conversion). During Interval I, the rate of polymerization increases with the increasing time of reaction and only one out of every 100-1000 micelles becomes a polymer particle. The number of particles nucleated per unit volume of water (*Np*) is proportional to the emulsifier concentration and initiator concentration to the 0.6 and 0.4 powers, respectively according to the Smith-Ewart theory. After the particle nucleation process is completed, this number remains relatively constant toward the end of

*The particle growth stage (Interval II):* After the particle nucleation process is completed, polymerization proceeds homogeneously in the polymer particles as the monomer concentration in the particles is maintained at a constant concentration by diffusion of monomer from the monomer droplets. The rate of polymerization in this stage is constant. In addition, during this stage, the number of monomer-swollen polymer particles and the monomer/polymer ratio remain constant. The monomer droplets decrease in size as the size of the polymeric particles increase. When monomer droplets completely disappear in the

Gardon, is called as **"micellar" or "heterogeneous" nucleation** [42].

polymerization.

This equation show that the polymerization rate depends on the square root of the initiation rate. If we make an arrangement on this equation by using Equation 2.9, we can say that the polymerization rate depends on the square root of the initiator concentration:

$$R\_p = k\_p \text{[}M\text{]} \left(\frac{fk\_d[I]}{k\_t}\right)^{\text{V}\_2} \tag{19}$$

In the emulsion polymerizations, the free-radical mechanism is very closely connected with the heterogeneous nature of the emulsion polymerization in which the micellar phase, the aqueous phase, the monomer droplet phase and the particle phase exist. Therefore, a number of mechanisms have been proposed for latex particle formation. The most important qualitative mechanism of emulsion polymerization was proposed by Harkins in 1945 and 1946 [38-39]. The following main premises of this mechanism were taken by Smith and Ewart. They managed to obtain first quantitative theory, which consist of equations for determining the rate of polymerization and the number of latex particles, for emulsion polymerization [40]. These theories have been applied only to the emulsion polymerization of "hydrophobic monomers" (such as sytrene) in the presence of water-soluble initiators and nonspecific, micelle-forming emulsifiers at concentrations significantly exceeding the critical micelle concentration. A schematic representation of the Harkins theory is illustrated in Figure 1 [11,41]. Such a system contains the emulsified monomer droplets (ca. 1-10 μm in diameter) dispersed in the continuous aqueous phase with the aid of an emulsifier at the very beginning of polymerization. Monomer-swollen micelles (5-10 nm in diameter) also exist in this system provided that the concentration of emulsifier in the aqueous phase is above (CMC). Only a small fraction (approximately 1%) of the total monomer is actually solubilized by the micelles and only an insignificant amount of monomer (with hydrophobic monomers such as styrene; about 0.04%) is dissolved by water. Most of the monomer molecules are in the monomer droplets which act as a reservoir of monomers during polymerization. Thus, the system prior to initiation contains mainly three parts: the water phase, large monomer droplets dispersed throughout the water phase, and the emulsifier micelles containing solubilized monomer. In addition, a very small amount of molecularly dissolved emulsifier and monomer-free micelles may exist (Figure 1.a).

After the emulsion of the monomer phase in the water phase and the presence of the emulsifier micelles established, the polymerization is initiated by the addition of initiator. According to the theories proposed by Harkins and Smith and Ewart, conventional emulsion polymerization mechanism occurs into three intervals including the initial (particle formation or nucleation) stage, the particle growth stage and the completion stage.

*The initial stage (Interval I):* This stage is also called as "*particle formation*" or "*nucleation*". With the addition of initiator to the reaction mixture, the free-radicals which initiate the polymerization are generated in the aqueous phase and diffuse into monomer-swollen micelles. These micelles are the principal locus for the initiation of polymer particle nuclei. In other words, they act as a meeting place for the hydrophobic monomer and the watersoluble initiator. Since they exhibit an extremely large oil-water interfacial area for diffusing of free-radicals and have high monomer concentration. On the other hand, a small amount of particle initiation can occur within the continuous aqueous phase. Monomer molecules dissolved in this phase are first polymerized by waterborne free-radicals. This would result in the increased hdrophobicity of oligomeric radicals. When a critical chain length is achieved, these oligomeric radicals become so hydrophobic that they show a strong tendency to enter the monomer-swollen micelles and then continue to propagate by reacting with those monomer molecules. But this nucleation becomes less significant as the amount of micellar emulsifier in the system increases. The amount of polymerization occurring in the monomer droplets is regarded as being a very minor proportion of the whole because of their small surface area for diffusing of the free-radicals. As a result, monomer-swollen micelles are favored as the sites of the nucleation of polymer particles. Therefore, this nucleation mechanism, proposed by Harkins and Smith and Ewart and modified by Gardon, is called as **"micellar" or "heterogeneous" nucleation** [42].

46 Polymer Science

1 2

1

(18)

(19)

*t*

*k*

2 [ ] [ ] *d*

*t*

*k*

[ ] 2 *i*

This equation show that the polymerization rate depends on the square root of the initiation rate. If we make an arrangement on this equation by using Equation 2.9, we can say that the

*p p*

polymerization rate depends on the square root of the initiator concentration:

*p p*

dissolved emulsifier and monomer-free micelles may exist (Figure 1.a).

After the emulsion of the monomer phase in the water phase and the presence of the emulsifier micelles established, the polymerization is initiated by the addition of initiator. According to the theories proposed by Harkins and Smith and Ewart, conventional emulsion polymerization mechanism occurs into three intervals including the initial (particle formation or nucleation) stage, the particle growth stage and the completion stage. *The initial stage (Interval I):* This stage is also called as "*particle formation*" or "*nucleation*". With the addition of initiator to the reaction mixture, the free-radicals which initiate the polymerization are generated in the aqueous phase and diffuse into monomer-swollen

*fk I R kM*

In the emulsion polymerizations, the free-radical mechanism is very closely connected with the heterogeneous nature of the emulsion polymerization in which the micellar phase, the aqueous phase, the monomer droplet phase and the particle phase exist. Therefore, a number of mechanisms have been proposed for latex particle formation. The most important qualitative mechanism of emulsion polymerization was proposed by Harkins in 1945 and 1946 [38-39]. The following main premises of this mechanism were taken by Smith and Ewart. They managed to obtain first quantitative theory, which consist of equations for determining the rate of polymerization and the number of latex particles, for emulsion polymerization [40]. These theories have been applied only to the emulsion polymerization of "hydrophobic monomers" (such as sytrene) in the presence of water-soluble initiators and nonspecific, micelle-forming emulsifiers at concentrations significantly exceeding the critical micelle concentration. A schematic representation of the Harkins theory is illustrated in Figure 1 [11,41]. Such a system contains the emulsified monomer droplets (ca. 1-10 μm in diameter) dispersed in the continuous aqueous phase with the aid of an emulsifier at the very beginning of polymerization. Monomer-swollen micelles (5-10 nm in diameter) also exist in this system provided that the concentration of emulsifier in the aqueous phase is above (CMC). Only a small fraction (approximately 1%) of the total monomer is actually solubilized by the micelles and only an insignificant amount of monomer (with hydrophobic monomers such as styrene; about 0.04%) is dissolved by water. Most of the monomer molecules are in the monomer droplets which act as a reservoir of monomers during polymerization. Thus, the system prior to initiation contains mainly three parts: the water phase, large monomer droplets dispersed throughout the water phase, and the emulsifier micelles containing solubilized monomer. In addition, a very small amount of molecularly

*R R kM*

After nucleation, monomer-swollen micelles are transformed into polymer particles swollen with monomer. The monomers are then acquired to the particles continuously from monomer droplets by diffusion through the aqueous phase, because monomer has been consumed with in the reaction loci by the polymerization process. Thus, the micelles grow from tiny groups of emulsifier and monomer molecules to larger groups of polymer molecules held in emulsion by the action of the emulsifier molecules located on the exterior surfaces of the particles. This action of the emulsifiers for providing colloidal stability of the growing particle nuclei occurs by emulsifiers supplied from the aqueous phase; this in turn tends to leads to dissociation of micelles containing monomer in which polymerization has not yet started. With the continued adsorption of micellar emulsifiers on to growing particles, the micelles start to disappear (Figure 1.b). The particle nucleation stage (Interval I) ends with this disappearance of the micelles at relatively early in the reaction (e.g. between 10% and 20% conversion). During Interval I, the rate of polymerization increases with the increasing time of reaction and only one out of every 100-1000 micelles becomes a polymer particle. The number of particles nucleated per unit volume of water (*Np*) is proportional to the emulsifier concentration and initiator concentration to the 0.6 and 0.4 powers, respectively according to the Smith-Ewart theory. After the particle nucleation process is completed, this number remains relatively constant toward the end of polymerization.

*The particle growth stage (Interval II):* After the particle nucleation process is completed, polymerization proceeds homogeneously in the polymer particles as the monomer concentration in the particles is maintained at a constant concentration by diffusion of monomer from the monomer droplets. The rate of polymerization in this stage is constant. In addition, during this stage, the number of monomer-swollen polymer particles and the monomer/polymer ratio remain constant. The monomer droplets decrease in size as the size of the polymeric particles increase. When monomer droplets completely disappear in the

polymerization system (at 50-80% conversion), the particle growth stage (Interval II) ends (Figure 1.c). In this situation, the polymer particles contain all the unreacted monomer and essentially all of the emulsifier molecules are also attached to the surface of polymer particles.

Emulsion Polymerization:

Effects of Polymerization Variables on the Properties of Vinyl Acetate Based Emulsion Polymers 49

*The completion stage (Interval III):* This is the final stage of the reaction. In this stage, polymerization continues within the monomer-swollen polymer particles which were formed during Interval I, and persisted and grew during Interval II (Figure 1.d). In the ideal case, the number of reaction loci during this stage is essentially fixed at the number which had become formed at the end of Interval I. Whereas, the concentration of monomer in the reaction loci and the polymerization rate continues to decrease toward the end of polymerization.  The system now comprises a dispersion of small polymer particles

To calculate the rate of emulsion polymerization (*Rp*) of relatively water-insoluble monomers such as styrene and butadiene, Smith Ewart case 2 kinetics has been widely used

( /) *p p pA p*

where *kp* is the rate constant of propagation, *[Mp]* the concentration of monomer in the particles, *n* the average number of free radicals per particle, and *NA* the Avogadro number.

Other than micellar nucleation, many mechanisms have been proposed to explain the particle nucleation stage. The best-known alternative theory for particle nucleation is that of **"homogeneous nucleation"** which includes the formation of particle nuclei in the continuous aqueous phase. This theory is proposed by Priest, Roe and Fitch and Tsai, and extended by Hansen and Ugelstad (HUFT) describes the emulsion polymerization of watersolubble monomers such as vinyl acetate and acrylonitrile, their water solubility though low (< 3%) is much in excess of the amount of monomer which may be solubilized by the emulsifier [43-48]. It is also the only mechanism which can apply to monomers of low watersolubility, such as styrene, in emulsifier-free reaction system, and also in reaction system which contain a micellizing emulsifier but at such a concentration that is below the CMC. When the monomers are somewhat soluble in the continuous phase, emulsifier micelles have little influence on particle formation. Emulsifier may be required, however, to ensure

colloidal stability of the product as it is formed and subsequently "on the shell".

Initially, free-radicals are generated in the aqueous phase by the thermal decomposition of initiator and they can grow by polymerization with those monomer molecules dissolved in the aqueous phase. When a growing oligomer reaches to critical chain lengths, it becomes water-insoluble. The water-insoluble radical then collapses upon itself and becomes effectively a separate phase. The primary particles thus formed provide a potential reaction locus which has within it an active growing free-radical if monomer molecules are available. Replenishment of monomer to the particles takes place by diffusing from the monomer droplets through the continuous phase. Indeed, the collapsed growing oligomer can be regarded as being similar to a emulsifier micelle. The oligomer is to some extent surfaceactive, because it incorporates both a hydrophilic moiety derived from the water-soluble initiator and hydrophobic units derived from the monomer molecules. The particles also

*R k M nN N* (20)

stabilized with the molecules of the original emulsifiers (Figure 1.e).

[40]:

**Figure 1.** Schematic representation for the mechanism of emulsion polymerization [11,41]

*The completion stage (Interval III):* This is the final stage of the reaction. In this stage, polymerization continues within the monomer-swollen polymer particles which were formed during Interval I, and persisted and grew during Interval II (Figure 1.d). In the ideal case, the number of reaction loci during this stage is essentially fixed at the number which had become formed at the end of Interval I. Whereas, the concentration of monomer in the reaction loci and the polymerization rate continues to decrease toward the end of polymerization.  The system now comprises a dispersion of small polymer particles stabilized with the molecules of the original emulsifiers (Figure 1.e).

48 Polymer Science

particles.

polymerization system (at 50-80% conversion), the particle growth stage (Interval II) ends (Figure 1.c). In this situation, the polymer particles contain all the unreacted monomer and essentially all of the emulsifier molecules are also attached to the surface of polymer

(a) (b)

(c) (d)

**Figure 1.** Schematic representation for the mechanism of emulsion polymerization [11,41]

(e)

To calculate the rate of emulsion polymerization (*Rp*) of relatively water-insoluble monomers such as styrene and butadiene, Smith Ewart case 2 kinetics has been widely used [40]:

$$R\_p = k\_p \boxed{M}\_p \left( \eta N\_p \,/\, N\_A \right) \tag{20}$$

where *kp* is the rate constant of propagation, *[Mp]* the concentration of monomer in the particles, *n* the average number of free radicals per particle, and *NA* the Avogadro number.

Other than micellar nucleation, many mechanisms have been proposed to explain the particle nucleation stage. The best-known alternative theory for particle nucleation is that of **"homogeneous nucleation"** which includes the formation of particle nuclei in the continuous aqueous phase. This theory is proposed by Priest, Roe and Fitch and Tsai, and extended by Hansen and Ugelstad (HUFT) describes the emulsion polymerization of watersolubble monomers such as vinyl acetate and acrylonitrile, their water solubility though low (< 3%) is much in excess of the amount of monomer which may be solubilized by the emulsifier [43-48]. It is also the only mechanism which can apply to monomers of low watersolubility, such as styrene, in emulsifier-free reaction system, and also in reaction system which contain a micellizing emulsifier but at such a concentration that is below the CMC. When the monomers are somewhat soluble in the continuous phase, emulsifier micelles have little influence on particle formation. Emulsifier may be required, however, to ensure colloidal stability of the product as it is formed and subsequently "on the shell".

Initially, free-radicals are generated in the aqueous phase by the thermal decomposition of initiator and they can grow by polymerization with those monomer molecules dissolved in the aqueous phase. When a growing oligomer reaches to critical chain lengths, it becomes water-insoluble. The water-insoluble radical then collapses upon itself and becomes effectively a separate phase. The primary particles thus formed provide a potential reaction locus which has within it an active growing free-radical if monomer molecules are available. Replenishment of monomer to the particles takes place by diffusing from the monomer droplets through the continuous phase. Indeed, the collapsed growing oligomer can be regarded as being similar to a emulsifier micelle. The oligomer is to some extent surfaceactive, because it incorporates both a hydrophilic moiety derived from the water-soluble initiator and hydrophobic units derived from the monomer molecules. The particles also may grow by limited coagulation of the relatively unstable primary particles [48-49]. The coagulation of these particles can occur with already-existing particles or other primary particles in the earliest (the first few tens of seconds) stage of the reaction. The particles formed by coagulation are now a potential reaction locus where the polymerization continues in the presence of further free-radical as well as monomer molecules. Colloidal stability of the collapsed oligomers and the growing particles is regulated by the amount of emulsifier adsorbed on their surfaces as well as by any other stabilizing group, ionic or nonionic, introduced by functional comonomers, initiator fragments or by chain transfer to molecules. The emulsifiers come from those dissolved in the aqueous phase and those adsorbed on the monomer droplet surfaces. If emulsifier micelles are present, then these are regarded as reservoirs of emulsifier molecules, dissociating as required to provide stabilizer.

The basic principle of this nucleation theory is that the formation of primary particles takes place up to the point where the rate of formation of the radicals in the aqueous phase is equal to the rate of their disappearing via capture of radicals by swollen micelles-if presentinitially and by particles already formed (Figure 2, [14]), and via coagulation.

According to this principle, the qualitative kinetic equation developed by Fitch and Tsai is:

$$
\left(\frac{dN}{dt}\right) = bR\_{\bar{n}w} - R\_c - R\_f \tag{21}
$$

Emulsion Polymerization:

Effects of Polymerization Variables on the Properties of Vinyl Acetate Based Emulsion Polymers 51

two effects. In the other hand, the positively skewed implies that the rate of particle nucleation increases with increasing time, and Feeney, Napper and Gilbert have explained

Oil-in-water emulsion polymerization systems are typically classified as possessing the characteristics of one of three types of emulsions: *macro-emulsions*, *mini-emulsions* or *microemulsions*. These emulsions are the initial systems for emulsion polymerization. There are quite differences between these systems in some aspects such as the size of the droplets (i.e. the discontinuous or dispersed phase), the interfacial area of the droplets, the particle

*Macro-emulsion polymerizations:* The conventional emulsion polymerization is referred as macro-emulsion polymerization. In this chapter, all explanations included so far relate to macro-emulsion polymerization. It is initially composed of a monomer emulsion of relatively large (1-100 μm) monomer droplets and significant free or micellar emulsifier. This emulsion is thermodynamically unstable, but kinetically stable. Phase separation is rapid unless the system is well agitated. In macro-emulsion polymerizations, the nucleation takes place outside the monomer droplets which generally do not contribute to the particle nucleation due to their very small droplet surface area. The monomer droplets act as only monomer reservoirs which supply the monomers to the polymerization loci through the

*Micro-emulsion polymerization:* In micro-emulsion polymerization, the initial system is microemulsion which consist of monomer droplets (varying from 10 to 100 nm) dispersed in water with the aid of a classical emulsifier (e.g. sodium dodecyl sulfate, SLS) and a "cosurfactant" such a low molar mass alcohol (pentanol or hexanol). Micro-emulsions are thermodynamically stable and optically one-phase solution. There is an excessive amount of emulsifier in these emulsions. Therefore, they are concentrated systems of micelles and the micelles exist throughout the reaction. One of the most interesting aspects of these micelles is their ability to accommodate monomer molecules. Furthermore, their high total surface area relative to nucleated particles implies the monomer-swollen micelles preferentially capture primary radicals generated in the continuous aqueous phase. Then the probability

that this skewed is a result of the coagulative nucleation.

**Figure 2.** Capture of radicals by a particle in homogeneous nucleation [14]

**2.3. Other types of emulsion polymerization**

nucleation mechanism and the stability of the emulsion.

aqueous phase.

where *t* is the reaction time, *N* the number of particles, *b* a parameter that takes into account the aggregation of oligomeric radicals, *Riw* the effective rate of initiation or free-radical generation in the aqueous phase, *Rc* the rate of capture of free-radicals, and *Rf* the rate of coagulation of the particles.

Feeney, Napper and Gilbert proposed a different particle nucleation theory, which resembles homogeneous nucleation [50]. They showed that particle size distributions during particle formation (Interval I) were positively skewed, confirming the role of coagulation.  They also have provided evidence that there can be coagulation even when the initial emulsifier concentration is above the CMC. It is possible that so many particles called "precursor" could be formed probably by homogeneous nucleation. Their size could be too small, and hence their surface area so much during growth, that they 'run out of' sufficient stabilizer providing their colloidal stability. This would result in coagulation in which the volume growth of the precursor particles by coagulation is much faster than that by propogation reactions. When these particles are sufficiently large to absorb appreciable amounts of monomer, "mature" primary latex particles occur. Monomer within the mature primary particles polymerizes more quickly than it those within the precursor particles. Because, the higher surface area of the precursor particles reduce the equilibrium swelling of the polymer by monomer, and hence the monomer concentration decreases. The smaller particles also can cause to exit of the free-radicals from the particles more easily. Consequently, the polymerization rate of the precursor particles decreases with increasing time due to these two effects. In the other hand, the positively skewed implies that the rate of particle nucleation increases with increasing time, and Feeney, Napper and Gilbert have explained that this skewed is a result of the coagulative nucleation.

**Figure 2.** Capture of radicals by a particle in homogeneous nucleation [14]

#### **2.3. Other types of emulsion polymerization**

50 Polymer Science

coagulation of the particles.

may grow by limited coagulation of the relatively unstable primary particles [48-49]. The coagulation of these particles can occur with already-existing particles or other primary particles in the earliest (the first few tens of seconds) stage of the reaction. The particles formed by coagulation are now a potential reaction locus where the polymerization continues in the presence of further free-radical as well as monomer molecules. Colloidal stability of the collapsed oligomers and the growing particles is regulated by the amount of emulsifier adsorbed on their surfaces as well as by any other stabilizing group, ionic or nonionic, introduced by functional comonomers, initiator fragments or by chain transfer to molecules. The emulsifiers come from those dissolved in the aqueous phase and those adsorbed on the monomer droplet surfaces. If emulsifier micelles are present, then these are regarded as reservoirs of emulsifier molecules, dissociating as required to provide stabilizer. The basic principle of this nucleation theory is that the formation of primary particles takes place up to the point where the rate of formation of the radicals in the aqueous phase is equal to the rate of their disappearing via capture of radicals by swollen micelles-if present-

initially and by particles already formed (Figure 2, [14]), and via coagulation.

*dt*

According to this principle, the qualitative kinetic equation developed by Fitch and Tsai is:

*dN bR R R*

where *t* is the reaction time, *N* the number of particles, *b* a parameter that takes into account the aggregation of oligomeric radicals, *Riw* the effective rate of initiation or free-radical generation in the aqueous phase, *Rc* the rate of capture of free-radicals, and *Rf* the rate of

Feeney, Napper and Gilbert proposed a different particle nucleation theory, which resembles homogeneous nucleation [50]. They showed that particle size distributions during particle formation (Interval I) were positively skewed, confirming the role of coagulation.  They also have provided evidence that there can be coagulation even when the initial emulsifier concentration is above the CMC. It is possible that so many particles called "precursor" could be formed probably by homogeneous nucleation. Their size could be too small, and hence their surface area so much during growth, that they 'run out of' sufficient stabilizer providing their colloidal stability. This would result in coagulation in which the volume growth of the precursor particles by coagulation is much faster than that by propogation reactions. When these particles are sufficiently large to absorb appreciable amounts of monomer, "mature" primary latex particles occur. Monomer within the mature primary particles polymerizes more quickly than it those within the precursor particles. Because, the higher surface area of the precursor particles reduce the equilibrium swelling of the polymer by monomer, and hence the monomer concentration decreases. The smaller particles also can cause to exit of the free-radicals from the particles more easily. Consequently, the polymerization rate of the precursor particles decreases with increasing time due to these

*iw c f*

(21)

Oil-in-water emulsion polymerization systems are typically classified as possessing the characteristics of one of three types of emulsions: *macro-emulsions*, *mini-emulsions* or *microemulsions*. These emulsions are the initial systems for emulsion polymerization. There are quite differences between these systems in some aspects such as the size of the droplets (i.e. the discontinuous or dispersed phase), the interfacial area of the droplets, the particle nucleation mechanism and the stability of the emulsion.

*Macro-emulsion polymerizations:* The conventional emulsion polymerization is referred as macro-emulsion polymerization. In this chapter, all explanations included so far relate to macro-emulsion polymerization. It is initially composed of a monomer emulsion of relatively large (1-100 μm) monomer droplets and significant free or micellar emulsifier. This emulsion is thermodynamically unstable, but kinetically stable. Phase separation is rapid unless the system is well agitated. In macro-emulsion polymerizations, the nucleation takes place outside the monomer droplets which generally do not contribute to the particle nucleation due to their very small droplet surface area. The monomer droplets act as only monomer reservoirs which supply the monomers to the polymerization loci through the aqueous phase.

*Micro-emulsion polymerization:* In micro-emulsion polymerization, the initial system is microemulsion which consist of monomer droplets (varying from 10 to 100 nm) dispersed in water with the aid of a classical emulsifier (e.g. sodium dodecyl sulfate, SLS) and a "cosurfactant" such a low molar mass alcohol (pentanol or hexanol). Micro-emulsions are thermodynamically stable and optically one-phase solution. There is an excessive amount of emulsifier in these emulsions. Therefore, they are concentrated systems of micelles and the micelles exist throughout the reaction. One of the most interesting aspects of these micelles is their ability to accommodate monomer molecules. Furthermore, their high total surface area relative to nucleated particles implies the monomer-swollen micelles preferentially capture primary radicals generated in the continuous aqueous phase. Then the probability

of capturing radicals by the micelles remains essentially one during the entire process and new particles thus are formed continuously. A growth in micellar size is always observed during the reaction due to the internal dynamics of micro-emulsions. This takes the form of either coagulation active and inactive micelles or the diffusion of monomer from the unreacted micelles to the nucleated particles. Reaction rates can be very fast. Finally, the small latex particles less than 50 nm are obtained from micro-emulsion polymerization. They on the average contain only one polymer molecule with average molecular weight exceeding one million [14-15,51].

Emulsion Polymerization:

Effects of Polymerization Variables on the Properties of Vinyl Acetate Based Emulsion Polymers 53

As well as *"inverse emulsion polymerization"*, there is also *"inverse micro-emulsion*

Three types of process are commonly used in carrying out the emulsion polymerization: *batch*, *semi-continuous*, and *continuous*. This classification is made according to the way in

*Batch process:* The batch-type process is the simplest method for effecting emulsion polymerization. All ingredients are placed in a reactor at the beginning of the reaction. The system is agitated, and heated to reaction temperature. Polymerization begins as soon as the initiator is added. Then, the reaction system is kept there by heating or cooling, as needed, and by agitating until the samples removed indicate the desired conversion of monomer to polymer. The only significant changes which can be made in such cases are to the reaction temperature, reactor design and the type and speed of agitation. Emulsion polymerization behavior in batch process can be divided into three intervals, as clearly explained in section 2.2: Interval I, free-radicals generated in the aqueous phase enter micelles and form new polymer particles. In Interval II, particles grow by continuously feeding of monomer from monomer droplets. In Interval III, polymerization continues in the monomer-swollen particles. During Interval III of a batch process, monomer concentrations in the polymer

It is commonly used in the laboratory to study reaction mechanism and kinetics, but most commercial latexes are not manufactured by this process because of their undesirable properties. This process has the important disadvantages that limited control is exerted over either monomer/polymer ratio in the reaction loci, or over heat transfer in the reaction, or over copolymer composition. Nevertheless, batch process has an important role, particularly

*Semi-continuous (or semi-batch) process:* This process is very versatile and is widely used, both industrially and in academic laboratories. Semi-continuous emulsion polymerization offers great degree of operational flexibility than batch or continuous processes. It allows one great control over the course of the polymerization, the rate of heat generation, and the properties and the morphology of the polymer latex particles. It also makes it possible to achieve relatively high polymer quality such as homogeneous chemical composition and particle

The semi-continuous emulsion polymerization processes is characterized by continued addition of reaction ingredients such as monomer, emulsifier, initiator, or water to the reaction system throughout the polymerization. In this emulsion polymerization process, two major types of feeds are used for the introduction of ingredients to the reactor; neat monomer feed (M) or monomer emulsion feed (ME). In M feed method, the feed contains only monomer and all the other ingredients are initially in the reactor. Otherwise, the major components of the ME feed are a monomer, a part from the emulsifier, and water. But it

*polymerization"* [15,51,55].

**2.4. Types of emulsion polymerization process**

particles and in the aqueous phase decrease with time.

in more fundamental studies.

size distribution.

which the Interval II and Interval III reactions are effected [29].

*Mini-emulsion polymerization:* Mini-emulsions are produced by dispersing monomer in water by means of vigorous mechanical agitation or homogenization using a mixed emulsifier system including a classical emulsifier and a water-insoluble "co-surfactant" such as a long chain fatty alcohol or alkane (e.g. cetyl alcohol or hexadecane). The stability of miniemulsions can continue for as little as days and as long as months. The polymerization of these emulsions can begin with submicrometre monomer droplets (from 50 to 500 nm). The long chain co-surfactants penetrate less the oil-water interface than the small monomer molecules, thus the emulsifier molecules move closer together, decreasing the interfacial area. Hence, the monomer droplets formed smaller size can become predominant particle nucleation loci provided that the total monomer droplet surface area becomes large enough to compete effectively with the continuous aqueous phase, in which particle nuclei are generated, for capturing waterborne free-radicals (monomer droplet nucleation). For propagation, the monomer is provided from within the polymerizing particles. Not all monomer droplets become polymer particles. Monomer droplets can be disappeared by another mechanism different from nucleation such as monomer diffusion to growing particles or by collision with polymer particles. No free, monomer-swollen micelles are present in this system since excess emulsifier has been adsorbed onto the large dropletwater interfacial area. The final polymer particles have almost the same size as the initial monomer droplets. Their size is often larger and their particle size distribution is broader than those obtained by conventional means of homogeneous or micellar nucleation [15,52- 54].

In contrast to these *oil-in-water emulsions*, it is possible that the emulsion polymerization can also be carried out with inverse emulsions. *Inverse (water-in-oil) emulsion polymerization* in which an aqueous solution of a water miscible hydrophilic monomer such as acrylamide, acrylic acid, or methacrylic acid is dispersed in a continuous hydrophobic oil phase with the aid of a water-in-oil emulsifier such as sorbitan mono-oleate or -stearate. The emulsifier is ordinarily above the CMC. Polymerization can be initiated with either oil-soluble or watersoluble initiators. If an oil-soluble initiator is used, the system is an almost exact 'mirrorimage' of a conventional emulsion polymerization system. The final latex is a colloidal dispersion of submicroscopic, water-swollen particles in oil. This type of emulsion polymerization enables the preparation of high molecular weights water-soluble polymers at rapid reaction rates. It is also possible that the water-swollen polymer particles produced by this emulsion polymerization transfer to aqueous phase rapidly by inversion of the latex. As well as *"inverse emulsion polymerization"*, there is also *"inverse micro-emulsion polymerization"* [15,51,55].

#### **2.4. Types of emulsion polymerization process**

52 Polymer Science

54].

exceeding one million [14-15,51].

of capturing radicals by the micelles remains essentially one during the entire process and new particles thus are formed continuously. A growth in micellar size is always observed during the reaction due to the internal dynamics of micro-emulsions. This takes the form of either coagulation active and inactive micelles or the diffusion of monomer from the unreacted micelles to the nucleated particles. Reaction rates can be very fast. Finally, the small latex particles less than 50 nm are obtained from micro-emulsion polymerization. They on the average contain only one polymer molecule with average molecular weight

*Mini-emulsion polymerization:* Mini-emulsions are produced by dispersing monomer in water by means of vigorous mechanical agitation or homogenization using a mixed emulsifier system including a classical emulsifier and a water-insoluble "co-surfactant" such as a long chain fatty alcohol or alkane (e.g. cetyl alcohol or hexadecane). The stability of miniemulsions can continue for as little as days and as long as months. The polymerization of these emulsions can begin with submicrometre monomer droplets (from 50 to 500 nm). The long chain co-surfactants penetrate less the oil-water interface than the small monomer molecules, thus the emulsifier molecules move closer together, decreasing the interfacial area. Hence, the monomer droplets formed smaller size can become predominant particle nucleation loci provided that the total monomer droplet surface area becomes large enough to compete effectively with the continuous aqueous phase, in which particle nuclei are generated, for capturing waterborne free-radicals (monomer droplet nucleation). For propagation, the monomer is provided from within the polymerizing particles. Not all monomer droplets become polymer particles. Monomer droplets can be disappeared by another mechanism different from nucleation such as monomer diffusion to growing particles or by collision with polymer particles. No free, monomer-swollen micelles are present in this system since excess emulsifier has been adsorbed onto the large dropletwater interfacial area. The final polymer particles have almost the same size as the initial monomer droplets. Their size is often larger and their particle size distribution is broader than those obtained by conventional means of homogeneous or micellar nucleation [15,52-

In contrast to these *oil-in-water emulsions*, it is possible that the emulsion polymerization can also be carried out with inverse emulsions. *Inverse (water-in-oil) emulsion polymerization* in which an aqueous solution of a water miscible hydrophilic monomer such as acrylamide, acrylic acid, or methacrylic acid is dispersed in a continuous hydrophobic oil phase with the aid of a water-in-oil emulsifier such as sorbitan mono-oleate or -stearate. The emulsifier is ordinarily above the CMC. Polymerization can be initiated with either oil-soluble or watersoluble initiators. If an oil-soluble initiator is used, the system is an almost exact 'mirrorimage' of a conventional emulsion polymerization system. The final latex is a colloidal dispersion of submicroscopic, water-swollen particles in oil. This type of emulsion polymerization enables the preparation of high molecular weights water-soluble polymers at rapid reaction rates. It is also possible that the water-swollen polymer particles produced by this emulsion polymerization transfer to aqueous phase rapidly by inversion of the latex. Three types of process are commonly used in carrying out the emulsion polymerization: *batch*, *semi-continuous*, and *continuous*. This classification is made according to the way in which the Interval II and Interval III reactions are effected [29].

*Batch process:* The batch-type process is the simplest method for effecting emulsion polymerization. All ingredients are placed in a reactor at the beginning of the reaction. The system is agitated, and heated to reaction temperature. Polymerization begins as soon as the initiator is added. Then, the reaction system is kept there by heating or cooling, as needed, and by agitating until the samples removed indicate the desired conversion of monomer to polymer. The only significant changes which can be made in such cases are to the reaction temperature, reactor design and the type and speed of agitation. Emulsion polymerization behavior in batch process can be divided into three intervals, as clearly explained in section 2.2: Interval I, free-radicals generated in the aqueous phase enter micelles and form new polymer particles. In Interval II, particles grow by continuously feeding of monomer from monomer droplets. In Interval III, polymerization continues in the monomer-swollen particles. During Interval III of a batch process, monomer concentrations in the polymer particles and in the aqueous phase decrease with time.

It is commonly used in the laboratory to study reaction mechanism and kinetics, but most commercial latexes are not manufactured by this process because of their undesirable properties. This process has the important disadvantages that limited control is exerted over either monomer/polymer ratio in the reaction loci, or over heat transfer in the reaction, or over copolymer composition. Nevertheless, batch process has an important role, particularly in more fundamental studies.

*Semi-continuous (or semi-batch) process:* This process is very versatile and is widely used, both industrially and in academic laboratories. Semi-continuous emulsion polymerization offers great degree of operational flexibility than batch or continuous processes. It allows one great control over the course of the polymerization, the rate of heat generation, and the properties and the morphology of the polymer latex particles. It also makes it possible to achieve relatively high polymer quality such as homogeneous chemical composition and particle size distribution.

The semi-continuous emulsion polymerization processes is characterized by continued addition of reaction ingredients such as monomer, emulsifier, initiator, or water to the reaction system throughout the polymerization. In this emulsion polymerization process, two major types of feeds are used for the introduction of ingredients to the reactor; neat monomer feed (M) or monomer emulsion feed (ME). In M feed method, the feed contains only monomer and all the other ingredients are initially in the reactor. Otherwise, the major components of the ME feed are a monomer, a part from the emulsifier, and water. But it

contains other ingredients. The main difference between the two types is the emulsifier concentration throughout the polymerization. The initiator can initially be charged or/and continuously fed during polymerization. By the continuous addition of the emulsifier, monomer, and initiator to the reaction mixture, the mechanisms (especially particle formation) and kinetics of the semi-continuous emulsion polymerization process become more complicated in comparison with the batch counterpart. Both types of feed can be added to the reactor at any desired time or feeding rate during the feed addition stage. Generally, two types of feed addition strategy have been applied: monomer-flooded and monomer-starved. In the monomer-flooded type, the rate of monomer addition is higher than the maximum polymerization rate attainable by the system. The monomer accumulates in the system as monomer droplets and the polymer particles are saturated with the monomer, as in Interval II of a batch process. In the monomer-starved type, the rate of addition is lower than the rate of polymerization and the polymerization reaction occurs in Interval III where particles are not swollen to their maximum size, leading to the production of small sized, high solid content latexes [56-66].

Emulsion Polymerization:

Effects of Polymerization Variables on the Properties of Vinyl Acetate Based Emulsion Polymers 55

flow in which the reacting mixture passes through the reactor without any forward or backward mixing. For the production of large amounts of the same product, the use of a CSTR may be preferable. In CSTR system, the reaction system is fed continuously to tank reactor, and from this reactor it is removed continuously at the same rate, the mixture in the tank being agitated to such an extent that it remains effectively homogeneous at all stage of the process. These reactors are characterized by isothermal, spatially uniform operation. There may be only one CSTR, or multiple CSTRs in a chain, the product from one being the feed for the next in the chain. The greater the numbers of CSTRs in a chain, the closer the properties approach those from a batch reaction. In such a system, residence time, which is defined as a finite time for remaining of the reaction system in the reactor, is important matter. Because, the performance of continuous flow reactor for emulsion polymerization in terms of conversion, particle concentration and particle size distribution strongly depends on the residence time distribution. Generally, conversion and particle number are lower and the particle size distribution is broader as compared to batch process. In particular, the particle nucleation stage is sensitive to residence time distribution [14,29,67]. Continuous emulsion polymerization process is useful for the production of commercial latexes. This process enables economical production of large volume, formation a highly uniform and well regulated product, and fewer problems with wall polymer buildup and coagulation. But, it allows less operational flexibility and less control on the product characteristics such

Besides of this classification including the above three processes, another classification is also made according to the way in which the reaction loci are formed. By this way, two types of reaction system are defined: *"ab initio emulsion polymerization"* and *"seeded emulsion*

*ab initio emulsion polymerization:* In this type reactions, the particle nucleation (the generation of reaction loci) proceed in a significant period (during the early stage) of the reaction by

*Seeded (multi-stage) emulsion polymerization:* In this reaction type, reaction loci are present in the initial system. The loci are formed by a separate reaction called as first stage of the emulsion polymerization. Thus, the particle nucleation stage of the reaction is eliminated by use of a pre-formed latex. Then, the pre-formed latex is introduced to the reaction mixture at the beginning. There must be enough seed particles to avoid new particles being subsequently nucleated. If the particle number is sufficiently high (typically, 1016 particles per liter is satisfactory), then the seed particles efficiently capture free-radical species from the aqueous phase and all primary particles that form by homogeneous nucleation (second stage of the emulsion polymerization). It is also possible that coagulation of tiny primary particles onto seed particles (heterocoagulation strongly affected by the surface charge on the seed particles) in the absence of emulsifier. When emulsifier is in the formulation, the amount of emulsifier must be just enough to maintain the colloidal stability of the seed latex particles as they grow through polymerization and/or coagulation with primary particles, but not so high as to generate new particles. In the second stage of the emulsion

mechanisms described as in section 2.2. No reaction loci are initially present.

as specific particle size distribution or particle morphologies [15].

*polymerization"* [29].

A semi-continuous process generally contains three successive operations: seeding batch stage (or preliminary batch), feed addition semi-continuous stage and finishing batch stage. Generally, a semi-continuous process starts with a seeding batch stage which is the most critical stage of a semi-continuous process. It controls the particle formation in the whole course of the reaction. Therefore, the distributions of ingredients between initial reactor charge and feed have a great effect on the particle formation. The time interval between initiation and the start of feeding, which is called the "pre-period" or "seeding time", will determine the duration of seeding batch. Further growth of polymer particles is achieved by absorption of the monomer from the feed. After the pre-period time, particle nucleation may be complete but, in some conditions, nucleation can continue during the feeding period. If no pre-period is allowed, the seeding proceeds during the feed addition stage. The feeding stage is generally known as the "growth stage" and is the only stage within the three stages defined above which is carried out semi-continuous wise. The finishing batch is carried out to reduce the amount of unreacted monomer remaining in the reaction mixture to a minimum [61,63-64].

Consequently, semi-continuous emulsion polymerization is an important process, which overcomes the disadvantages of the batch and continuous processes, for the manufacture of a variety of latex products because of its operational flexibility and, providing control on the polymerization and the properties of polymer and latex.

*Continuous process:* In this process, the reaction system is continuously fed to, and removed from, a suitable reactor at rates such that the total volume of system undergoing reaction at any instant is constant. There are two basic type reactors for effecting continuous emulsion polymerization: the continuous stirred-tank reactor (CSTR) and tubular reactor. In tubular system, the composition is constant with time at any given position in the reactor. They are generally unsatisfactory for industrial production because of the very long tube lengths required, the poor degree of mixing and the difficulties of cleaning. They also require plugflow in which the reacting mixture passes through the reactor without any forward or backward mixing. For the production of large amounts of the same product, the use of a CSTR may be preferable. In CSTR system, the reaction system is fed continuously to tank reactor, and from this reactor it is removed continuously at the same rate, the mixture in the tank being agitated to such an extent that it remains effectively homogeneous at all stage of the process. These reactors are characterized by isothermal, spatially uniform operation. There may be only one CSTR, or multiple CSTRs in a chain, the product from one being the feed for the next in the chain. The greater the numbers of CSTRs in a chain, the closer the properties approach those from a batch reaction. In such a system, residence time, which is defined as a finite time for remaining of the reaction system in the reactor, is important matter. Because, the performance of continuous flow reactor for emulsion polymerization in terms of conversion, particle concentration and particle size distribution strongly depends on the residence time distribution. Generally, conversion and particle number are lower and the particle size distribution is broader as compared to batch process. In particular, the particle nucleation stage is sensitive to residence time distribution [14,29,67]. Continuous emulsion polymerization process is useful for the production of commercial latexes. This process enables economical production of large volume, formation a highly uniform and well regulated product, and fewer problems with wall polymer buildup and coagulation. But, it allows less operational flexibility and less control on the product characteristics such as specific particle size distribution or particle morphologies [15].

54 Polymer Science

of small sized, high solid content latexes [56-66].

polymerization and the properties of polymer and latex.

minimum [61,63-64].

contains other ingredients. The main difference between the two types is the emulsifier concentration throughout the polymerization. The initiator can initially be charged or/and continuously fed during polymerization. By the continuous addition of the emulsifier, monomer, and initiator to the reaction mixture, the mechanisms (especially particle formation) and kinetics of the semi-continuous emulsion polymerization process become more complicated in comparison with the batch counterpart. Both types of feed can be added to the reactor at any desired time or feeding rate during the feed addition stage. Generally, two types of feed addition strategy have been applied: monomer-flooded and monomer-starved. In the monomer-flooded type, the rate of monomer addition is higher than the maximum polymerization rate attainable by the system. The monomer accumulates in the system as monomer droplets and the polymer particles are saturated with the monomer, as in Interval II of a batch process. In the monomer-starved type, the rate of addition is lower than the rate of polymerization and the polymerization reaction occurs in Interval III where particles are not swollen to their maximum size, leading to the production

A semi-continuous process generally contains three successive operations: seeding batch stage (or preliminary batch), feed addition semi-continuous stage and finishing batch stage. Generally, a semi-continuous process starts with a seeding batch stage which is the most critical stage of a semi-continuous process. It controls the particle formation in the whole course of the reaction. Therefore, the distributions of ingredients between initial reactor charge and feed have a great effect on the particle formation. The time interval between initiation and the start of feeding, which is called the "pre-period" or "seeding time", will determine the duration of seeding batch. Further growth of polymer particles is achieved by absorption of the monomer from the feed. After the pre-period time, particle nucleation may be complete but, in some conditions, nucleation can continue during the feeding period. If no pre-period is allowed, the seeding proceeds during the feed addition stage. The feeding stage is generally known as the "growth stage" and is the only stage within the three stages defined above which is carried out semi-continuous wise. The finishing batch is carried out to reduce the amount of unreacted monomer remaining in the reaction mixture to a

Consequently, semi-continuous emulsion polymerization is an important process, which overcomes the disadvantages of the batch and continuous processes, for the manufacture of a variety of latex products because of its operational flexibility and, providing control on the

*Continuous process:* In this process, the reaction system is continuously fed to, and removed from, a suitable reactor at rates such that the total volume of system undergoing reaction at any instant is constant. There are two basic type reactors for effecting continuous emulsion polymerization: the continuous stirred-tank reactor (CSTR) and tubular reactor. In tubular system, the composition is constant with time at any given position in the reactor. They are generally unsatisfactory for industrial production because of the very long tube lengths required, the poor degree of mixing and the difficulties of cleaning. They also require plugBesides of this classification including the above three processes, another classification is also made according to the way in which the reaction loci are formed. By this way, two types of reaction system are defined: *"ab initio emulsion polymerization"* and *"seeded emulsion polymerization"* [29].

*ab initio emulsion polymerization:* In this type reactions, the particle nucleation (the generation of reaction loci) proceed in a significant period (during the early stage) of the reaction by mechanisms described as in section 2.2. No reaction loci are initially present.

*Seeded (multi-stage) emulsion polymerization:* In this reaction type, reaction loci are present in the initial system. The loci are formed by a separate reaction called as first stage of the emulsion polymerization. Thus, the particle nucleation stage of the reaction is eliminated by use of a pre-formed latex. Then, the pre-formed latex is introduced to the reaction mixture at the beginning. There must be enough seed particles to avoid new particles being subsequently nucleated. If the particle number is sufficiently high (typically, 1016 particles per liter is satisfactory), then the seed particles efficiently capture free-radical species from the aqueous phase and all primary particles that form by homogeneous nucleation (second stage of the emulsion polymerization). It is also possible that coagulation of tiny primary particles onto seed particles (heterocoagulation strongly affected by the surface charge on the seed particles) in the absence of emulsifier. When emulsifier is in the formulation, the amount of emulsifier must be just enough to maintain the colloidal stability of the seed latex particles as they grow through polymerization and/or coagulation with primary particles, but not so high as to generate new particles. In the second stage of the emulsion polymerization, monomer can be added to reaction system including seed particles by three different methods: dynamic swelling, batch and semi-continuous. By dynamic swelling method, the second stage is carried out after the seed particles are swollen with the second monomer. In batch method where seed latex has a second monomer added in the second stage of the emulsion polymerization. For semi-continuous method, the second monomer is continuously added in monomer-starved conditions to the reaction system including the seed latex during the second stage. In addition, one or more types of monomer can be used in both stages of the seeded emulsion polymerization. For example, in ABS (acrylonitrile/butadiene/styrene) polymer, polybutadiene (PB) seed latex is polymerized with a mixture of styrene and acrylonitrile monomers added in the second stage of the emulsion polymerization. As a result, it is possible to produce polymer particles with a wide variety of morphologies such as 'dumb-bell' shaped, 'ice-cream cone' shaped, 'raspberry' shaped, or core-shell due to the multi-stage emulsion polymerization process enables changing the experimental conditions in a wide range. Furthermore, this process provides many advantages in the production of latex particles being uniform and having excellent monodispersity in size. It also has high production yields. Such features make these latexes more practical in final uses for a wide variety of application areas [14,29.68-69].

Emulsion Polymerization:

Effects of Polymerization Variables on the Properties of Vinyl Acetate Based Emulsion Polymers 57

value for styrene is 3.6x10-2 % [72]. Therefore, the initiation occurs in the aqueous phase and is explained by the *"homogeneous nucleation"* (as described in section 2.2). Another characteristic feature of VAc that affects the polymerization mechanism is its low reactivity and the correspondingly high reactivity of PVAc radicals in comparison with other vinyl monomers. This establishes the participation of the majority of components in the system in chain transfer during the polymerization of VAc. This has a substantial influence on the rate of polymerization, the molecular structure of the polymers, their branching, the tendency toward graft copolymerization, and also the tendency toward formation of significant amounts of gel fraction. In particular, the presence of a poly(vinyl alcohol), PVOH protective colloid in VAc emulsion polymerizations greatly affects branching and reaction mechanism. This agent is used as the principal surface-active substances in the system. More conventional emulsifiers may also be added to the system, but their role seems to be secondary that of this protective colloid. The chain transfer of PVAc to polymer, monomer and solvent (methanol) during emulsion polymerization in the absence of the PVOH is also a very important subject. As a result of these significant branching reactions of PVAc, there

Indeed, VAc has different features in comparison with other monomers in other respects than its water-solubility and the strong tendency of its radicals to the chain transfers. It has a high equilibrium monomer-polymer swelling ratio (values as great as 7:1). The heat of polymerization of VAc monomer is 210.5 kcal/mole [10]. Removing of the polymerization heat is of great importance in providing the control of the polymerization reaction. If not, a runaway exothermic reaction causes to uncontrollable boiling and consequent foaming or

All these specific features of VAc monomer require a controlled emulsion polymerization process to be useful this monomer in particular industrial practice. The most commonly used process in the industrial practice of VAc emulsion polymerization is the delayed addition method in semi-continuous process. In this method, 5-15% of the VAc monomer is added into the reactor with some of the ingredients such as water, emulsifier and initiator at start. After the particle-generating period is completed, the remaining ingredients are incrementally during the polymerization. In some cases there is also gradual addition of remaining neat monomer and initiator when all other water phase ingredients are in the initial reactor charge. Additionally, many variations can be made in this process (see also section 2.4, semi-continuous process). The delayed addition process avoids the coalescence of the monomer-swollen latex particles, thus attaining greater colloidal stability. Emulsion prepared in this manner also show smaller particle size than emulsions prepared by the batch process. In the other hand, the semi-continuous process produces a broader molar mass distribution than the batch process and a high molar mass fraction which is attributed

In the emulsion polymerization of VAc, the most commonly used initiators are the watersoluble, thermally decomposed, free-radical producing persulfates (peroxodisulfates) such as potassium-, sodium-, and ammonium-persulfate. Non-ionic and anionic emulsifiers (generally, mixtures of them) are the most widely preferred types because of improved

are considerable research results in literature on this subject [27,30,73-78].

to chain transfer reactions due to monomer-starved conditions [15].

destabilization.

#### **3. Emulsion polymerization of vinyl acetate**

The production of poly(vinyl acetate), PVAc latexes using poly(vinyl alcohol) as an emulsifier began in Germany during the mid-1930 [6]. Vinyl acetate, VAc emulsion polymerization recipes in use in Germany before and during World War II were originally disclosed in the BIOS (British Intelligence Objectives Subcommision) and the US FIAT (Field Intelligence Agency Technical) reports [7-8]. On the basis of these report information, manufacture of PVAc latex paints was begun in England in 1948. Afterwards, the production of PVAc latexes has continued to the present day, growing steadily over the years. During this period, too many studies have been done to explain the mechanism and kinetics of emulsion polymerization of VAc, to develop its polymerization conditions, and to improve the properties of PVAc latexes and their films. These subjects are still very important in both industrially and scientifically. Furthermore, VAc copolymers have been developed by using many kinds of comonomers such as ethylene, acrylates, maleates, vinyl chloride and versatic acid esters.

The industrial importance of VAc latexes necessitates the understanding of the mechanism and kinetics of VAc emulsion homopolymerization and copolymerizations with other comonomers by scientific communities as well as industrial communities. VAc is polymerized exclusively via free-radical polymerization. The emulsion homopolymerization mechanism of VAc is different from that of other vinyl monomers like styrene and butadiene. Although Smith-Ewart theory and related theories successfully explain the emulsion polymerization of nearly water-insoluble monomers, they are not fit the emulsion polymerization of VAc [4,70-71]. The most characteristic feature of VAc is its polarity and relatively high solubility in water in comparison with other hydrophobic monomers such as styrene. For example, the water-solubility value of VAc is 2.5% by weight at 20 oC, while this value for styrene is 3.6x10-2 % [72]. Therefore, the initiation occurs in the aqueous phase and is explained by the *"homogeneous nucleation"* (as described in section 2.2). Another characteristic feature of VAc that affects the polymerization mechanism is its low reactivity and the correspondingly high reactivity of PVAc radicals in comparison with other vinyl monomers. This establishes the participation of the majority of components in the system in chain transfer during the polymerization of VAc. This has a substantial influence on the rate of polymerization, the molecular structure of the polymers, their branching, the tendency toward graft copolymerization, and also the tendency toward formation of significant amounts of gel fraction. In particular, the presence of a poly(vinyl alcohol), PVOH protective colloid in VAc emulsion polymerizations greatly affects branching and reaction mechanism. This agent is used as the principal surface-active substances in the system. More conventional emulsifiers may also be added to the system, but their role seems to be secondary that of this protective colloid. The chain transfer of PVAc to polymer, monomer and solvent (methanol) during emulsion polymerization in the absence of the PVOH is also a very important subject. As a result of these significant branching reactions of PVAc, there are considerable research results in literature on this subject [27,30,73-78].

56 Polymer Science

polymerization, monomer can be added to reaction system including seed particles by three different methods: dynamic swelling, batch and semi-continuous. By dynamic swelling method, the second stage is carried out after the seed particles are swollen with the second monomer. In batch method where seed latex has a second monomer added in the second stage of the emulsion polymerization. For semi-continuous method, the second monomer is continuously added in monomer-starved conditions to the reaction system including the seed latex during the second stage. In addition, one or more types of monomer can be used in both stages of the seeded emulsion polymerization. For example, in ABS (acrylonitrile/butadiene/styrene) polymer, polybutadiene (PB) seed latex is polymerized with a mixture of styrene and acrylonitrile monomers added in the second stage of the emulsion polymerization. As a result, it is possible to produce polymer particles with a wide variety of morphologies such as 'dumb-bell' shaped, 'ice-cream cone' shaped, 'raspberry' shaped, or core-shell due to the multi-stage emulsion polymerization process enables changing the experimental conditions in a wide range. Furthermore, this process provides many advantages in the production of latex particles being uniform and having excellent monodispersity in size. It also has high production yields. Such features make these latexes

more practical in final uses for a wide variety of application areas [14,29.68-69].

The production of poly(vinyl acetate), PVAc latexes using poly(vinyl alcohol) as an emulsifier began in Germany during the mid-1930 [6]. Vinyl acetate, VAc emulsion polymerization recipes in use in Germany before and during World War II were originally disclosed in the BIOS (British Intelligence Objectives Subcommision) and the US FIAT (Field Intelligence Agency Technical) reports [7-8]. On the basis of these report information, manufacture of PVAc latex paints was begun in England in 1948. Afterwards, the production of PVAc latexes has continued to the present day, growing steadily over the years. During this period, too many studies have been done to explain the mechanism and kinetics of emulsion polymerization of VAc, to develop its polymerization conditions, and to improve the properties of PVAc latexes and their films. These subjects are still very important in both industrially and scientifically. Furthermore, VAc copolymers have been developed by using many kinds of comonomers such as ethylene, acrylates, maleates, vinyl

The industrial importance of VAc latexes necessitates the understanding of the mechanism and kinetics of VAc emulsion homopolymerization and copolymerizations with other comonomers by scientific communities as well as industrial communities. VAc is polymerized exclusively via free-radical polymerization. The emulsion homopolymerization mechanism of VAc is different from that of other vinyl monomers like styrene and butadiene. Although Smith-Ewart theory and related theories successfully explain the emulsion polymerization of nearly water-insoluble monomers, they are not fit the emulsion polymerization of VAc [4,70-71]. The most characteristic feature of VAc is its polarity and relatively high solubility in water in comparison with other hydrophobic monomers such as styrene. For example, the water-solubility value of VAc is 2.5% by weight at 20 oC, while this

**3. Emulsion polymerization of vinyl acetate**

chloride and versatic acid esters.

Indeed, VAc has different features in comparison with other monomers in other respects than its water-solubility and the strong tendency of its radicals to the chain transfers. It has a high equilibrium monomer-polymer swelling ratio (values as great as 7:1). The heat of polymerization of VAc monomer is 210.5 kcal/mole [10]. Removing of the polymerization heat is of great importance in providing the control of the polymerization reaction. If not, a runaway exothermic reaction causes to uncontrollable boiling and consequent foaming or destabilization.

All these specific features of VAc monomer require a controlled emulsion polymerization process to be useful this monomer in particular industrial practice. The most commonly used process in the industrial practice of VAc emulsion polymerization is the delayed addition method in semi-continuous process. In this method, 5-15% of the VAc monomer is added into the reactor with some of the ingredients such as water, emulsifier and initiator at start. After the particle-generating period is completed, the remaining ingredients are incrementally during the polymerization. In some cases there is also gradual addition of remaining neat monomer and initiator when all other water phase ingredients are in the initial reactor charge. Additionally, many variations can be made in this process (see also section 2.4, semi-continuous process). The delayed addition process avoids the coalescence of the monomer-swollen latex particles, thus attaining greater colloidal stability. Emulsion prepared in this manner also show smaller particle size than emulsions prepared by the batch process. In the other hand, the semi-continuous process produces a broader molar mass distribution than the batch process and a high molar mass fraction which is attributed to chain transfer reactions due to monomer-starved conditions [15].

In the emulsion polymerization of VAc, the most commonly used initiators are the watersoluble, thermally decomposed, free-radical producing persulfates (peroxodisulfates) such as potassium-, sodium-, and ammonium-persulfate. Non-ionic and anionic emulsifiers (generally, mixtures of them) are the most widely preferred types because of improved

compatibility with negatively charged PVAc particles as a result of persulfate initiator fragments. The use of protective colloids such as PVOH and hydroxyethyl cellulose (HEC) is common in the industrial emulsion polymerization of VAc. These water-soluble polymers can be used in the presence of emulsifier or in the emulsifier-free polymerization for the production of PVAc latexes and stable latexes can be made with only these protective colloids. The grafting reactions also take place between these protective colloids and VAc radicals, which influence the final product properties such as molar mass, viscosity and particle morphology. The VAc emulsion system is sensitive to changes of pH and the optimum pH range (pH=4.5—5.5) can be generally obtained by using sodium bicarbonate buffer system.

Emulsion Polymerization:

Effects of Polymerization Variables on the Properties of Vinyl Acetate Based Emulsion Polymers 59

**4. Effects of polymerization variables on the properties of vinyl acetate**

VAc monomer is a polar and reactive, and has the characteristic features. The significant differences between VAc and the comonomers lead to difficulties during copolymerization when the VAc is copolymerized with less polar and more reactive monomers. The emulsion copolymerization of VAc with the comonomers requires the special treatments. Other properties such as the copolymer structure, the particle morphology, and the colloidal, physical and film properties of the copolymer latex are also affected from this situation. In order to prevent potential problems and produce copolymer emulsion polymers in homogeneous copolymer structure and desired properties, the various processes and different ingredient systems are applied for VAc copolymerization systems. The major copolymerization systems of VAc and, the effects of copolymerization variables on the course of polymerization and the properties of emulsion copolymers are given in detail

One of the most important industrial latexes is the vinyl acetate/n-butyl acrylate (VAc/BuA) copolymer latex. This copolymer latex is utilized extensively in interior and exterior paints and is superior to either homopolymer alone. The main features of these monomers are: reactivity ratios (rVAc=0.05 and rBuA=5.5), water solubilities (25 g/L for VAc and 1-1.5 g/L for BuA, at 20 oC), and glass transition temperatures (Tg (PVAc) =32 oC and Tg (PBuA) = –54 oC). The presence of BuA in VAc emulsion copolymerizations results in internally plasticized copolymers with MFFTs in the ambient temperature range. BuA also imparts softness and tackiness, and thus the durability of VAc copolymer increases. Although polyacrylates and polymethacrylates are less susceptible to hydrolysis than the PVAc, VAc/BuA emulsion copolymers show sensibility to hydrolysis. In industry, 15-25% by weight of BuA is

The emulsion polymerization process types, especially batch and semi-continuous processes, are very effective on the VAc/BuA copolymerization and the obtained copolymers. In batch and semi-continuous emulsion processes of VAc/BuA comonomer mixtures having various compositions, homogeneous copolymer compositions are obtained only by semi-continuous process. In contrast, batch process produces the VAc/BuA latexes in heterogeneous copolymer composition. Due to the significantly differences in water solubility and reactivity ratio of this monomer couple, the semi-continuous process provides better control over compositional heterogeneity than batch process for this monomer couple [27,79-82]. The copolymer latexes produced by batch process have a larger average particle size (PS) and narrower particle size distribution (PSD) than the latexes produced by semicotinuous process. By increasing of BuA content in comonomer mixture the average particle size of semi-continuous latexes decreases, whereas it is independent of comonomer composition for batch-latexes [27,80,82-86]. In addition, the particle structures of batchlatexes have a larger BuA-rich core surrounded by a PVAc-rich shell, indicating heterogeneous structure, than the semi-continues latex particles [80]. Also, the ratio of each monomer on particle surface depending on the process type and copolymer composition

**based emulsion polymers**

below.

preferred.

As a result of the emulsion polymerization of VAc monomer, an amorphous, non-crystalline and thermoplastic polymer is obtained. Poly(vinyl acetate) is soluble in alcohols, ketones, aromatic hydrocarbons and ethers. It can be also solubilized in emulsifier solutions. It absorbs 3 to 6 wt% water between 20 to 70 oC within 24 hrs. Moreover, in the presence of water, it can hydrolyze to form vinyl alcohol units and acetic acid, or the acetate of the basic cation. The minimum film forming temperature (MFFT), the glass transition temperature (Tg) and the mechanical properties of the PVAc depend on the molecular weight. For medium molecular weight, its Tg is approximately 30 oC and its MFFT is approximately 20 oC. Its Young modulus is 600 N/mm2 at 25 oC with 50% relative humidity. The tensile strength and the elongation at break of PVAc are between 29.4—49.0 N/mm2 and 10—20% at 20 oC, respectively [30]. These properties depend on not only the molecular weight of the polymer, but also the emulsion polymerization type, the ingredients of the polymerization and the particle morphology of the polymer. The thermal degradation of PVAc occurs at 150-220 oC. PVAc is brittle on cooling below room temperature, i.e., at 10-15 oC [30].

Nevertheless, some of these properties of the PVAc make the VAc homopolymer latexes and its films unsuitable for many applications. For example, its films have low resistance against water, alkaline, and hydrolysis. They show poor mechanical properties. Tg and MFFT values of this homopolymer also constitute the major problems in its applications because the MFFT is too high for this polymer to perform as an effective binder for pigments and fillers at normal ambient temperatures. While the Tg is too low for the polymer to be useful as a rigid plastic at normal ambient temperatures, the same value is too high for application as a binder and an adhesive at the same temperatures. Due to these properties of the VAc homopolymer, VAc is copolymerized with other monomers such as ethylene, n-ethyl acrylate, n-butyl acrylate, 2-ethylhexyl acrylate, methyl methacrylate, vinyl chloride, vinyl propionate, vinyl versatate, maleates (dibutyl malate), fumarates, and acrylonitrile to improve the poor properties of this polymer. Terpolymers of VAc are also widely produced. The selection of comonomers to be used to produce VAc copolymer latexes for any given application depends principally upon the functional suitability of the comonomer and its coast. As well as the VAc homopolymer latex, The VAc based copolymer/terolymer latexes are widely used for exterior and interior architectural coatings, adhesives, textile and paper industry, and numerous other applications.

### **4. Effects of polymerization variables on the properties of vinyl acetate based emulsion polymers**

58 Polymer Science

buffer system.

compatibility with negatively charged PVAc particles as a result of persulfate initiator fragments. The use of protective colloids such as PVOH and hydroxyethyl cellulose (HEC) is common in the industrial emulsion polymerization of VAc. These water-soluble polymers can be used in the presence of emulsifier or in the emulsifier-free polymerization for the production of PVAc latexes and stable latexes can be made with only these protective colloids. The grafting reactions also take place between these protective colloids and VAc radicals, which influence the final product properties such as molar mass, viscosity and particle morphology. The VAc emulsion system is sensitive to changes of pH and the optimum pH range (pH=4.5—5.5) can be generally obtained by using sodium bicarbonate

As a result of the emulsion polymerization of VAc monomer, an amorphous, non-crystalline and thermoplastic polymer is obtained. Poly(vinyl acetate) is soluble in alcohols, ketones, aromatic hydrocarbons and ethers. It can be also solubilized in emulsifier solutions. It absorbs 3 to 6 wt% water between 20 to 70 oC within 24 hrs. Moreover, in the presence of water, it can hydrolyze to form vinyl alcohol units and acetic acid, or the acetate of the basic cation. The minimum film forming temperature (MFFT), the glass transition temperature (Tg) and the mechanical properties of the PVAc depend on the molecular weight. For medium molecular weight, its Tg is approximately 30 oC and its MFFT is approximately 20 oC. Its Young modulus is 600 N/mm2 at 25 oC with 50% relative humidity. The tensile strength and the elongation at break of PVAc are between 29.4—49.0 N/mm2 and 10—20% at 20 oC, respectively [30]. These properties depend on not only the molecular weight of the polymer, but also the emulsion polymerization type, the ingredients of the polymerization and the particle morphology of the polymer. The thermal degradation of PVAc occurs at

150-220 oC. PVAc is brittle on cooling below room temperature, i.e., at 10-15 oC [30].

industry, and numerous other applications.

Nevertheless, some of these properties of the PVAc make the VAc homopolymer latexes and its films unsuitable for many applications. For example, its films have low resistance against water, alkaline, and hydrolysis. They show poor mechanical properties. Tg and MFFT values of this homopolymer also constitute the major problems in its applications because the MFFT is too high for this polymer to perform as an effective binder for pigments and fillers at normal ambient temperatures. While the Tg is too low for the polymer to be useful as a rigid plastic at normal ambient temperatures, the same value is too high for application as a binder and an adhesive at the same temperatures. Due to these properties of the VAc homopolymer, VAc is copolymerized with other monomers such as ethylene, n-ethyl acrylate, n-butyl acrylate, 2-ethylhexyl acrylate, methyl methacrylate, vinyl chloride, vinyl propionate, vinyl versatate, maleates (dibutyl malate), fumarates, and acrylonitrile to improve the poor properties of this polymer. Terpolymers of VAc are also widely produced. The selection of comonomers to be used to produce VAc copolymer latexes for any given application depends principally upon the functional suitability of the comonomer and its coast. As well as the VAc homopolymer latex, The VAc based copolymer/terolymer latexes are widely used for exterior and interior architectural coatings, adhesives, textile and paper VAc monomer is a polar and reactive, and has the characteristic features. The significant differences between VAc and the comonomers lead to difficulties during copolymerization when the VAc is copolymerized with less polar and more reactive monomers. The emulsion copolymerization of VAc with the comonomers requires the special treatments. Other properties such as the copolymer structure, the particle morphology, and the colloidal, physical and film properties of the copolymer latex are also affected from this situation. In order to prevent potential problems and produce copolymer emulsion polymers in homogeneous copolymer structure and desired properties, the various processes and different ingredient systems are applied for VAc copolymerization systems. The major copolymerization systems of VAc and, the effects of copolymerization variables on the course of polymerization and the properties of emulsion copolymers are given in detail below.

One of the most important industrial latexes is the vinyl acetate/n-butyl acrylate (VAc/BuA) copolymer latex. This copolymer latex is utilized extensively in interior and exterior paints and is superior to either homopolymer alone. The main features of these monomers are: reactivity ratios (rVAc=0.05 and rBuA=5.5), water solubilities (25 g/L for VAc and 1-1.5 g/L for BuA, at 20 oC), and glass transition temperatures (Tg (PVAc) =32 oC and Tg (PBuA) = –54 oC). The presence of BuA in VAc emulsion copolymerizations results in internally plasticized copolymers with MFFTs in the ambient temperature range. BuA also imparts softness and tackiness, and thus the durability of VAc copolymer increases. Although polyacrylates and polymethacrylates are less susceptible to hydrolysis than the PVAc, VAc/BuA emulsion copolymers show sensibility to hydrolysis. In industry, 15-25% by weight of BuA is preferred.

The emulsion polymerization process types, especially batch and semi-continuous processes, are very effective on the VAc/BuA copolymerization and the obtained copolymers. In batch and semi-continuous emulsion processes of VAc/BuA comonomer mixtures having various compositions, homogeneous copolymer compositions are obtained only by semi-continuous process. In contrast, batch process produces the VAc/BuA latexes in heterogeneous copolymer composition. Due to the significantly differences in water solubility and reactivity ratio of this monomer couple, the semi-continuous process provides better control over compositional heterogeneity than batch process for this monomer couple [27,79-82]. The copolymer latexes produced by batch process have a larger average particle size (PS) and narrower particle size distribution (PSD) than the latexes produced by semicotinuous process. By increasing of BuA content in comonomer mixture the average particle size of semi-continuous latexes decreases, whereas it is independent of comonomer composition for batch-latexes [27,80,82-86]. In addition, the particle structures of batchlatexes have a larger BuA-rich core surrounded by a PVAc-rich shell, indicating heterogeneous structure, than the semi-continues latex particles [80]. Also, the ratio of each monomer on particle surface depending on the process type and copolymer composition effects hydrolysis and electrolyte resistance of the latexes [27,82]. The broader molecular weight distribution (MWD) with bimodal character is observed for semi-continuous copolymers. The MWD of batch copolymers are broad, but they are narrower and in unimodal character in comparison to those of semi-continuous copolymers. This results for both processes indicates the excessive branching reactions [27,82-85,87]. When the film properties of VAc/BuA copolymer latexes of various copolymer composition are examined, it is seen that the semi-continuous process provide better properties to copolymer films such as filming ability and film homogeneity (examined according to the Tg and surface analyzes) than the batch process [27,88]. The homogeneity influences hardness and adhesive properties of latexes as well as copolymer composition, and hardness decreases with increasing homogeneity [79]. The thermodynamic work of adhesion decreases with increasing BuA content for semi-continuous copolymer films [86]. In contrast, tensile properties of the batch copolymer films show a higher ultimate tensile strength, higher Young's modulus, and lower percent elongation to break compared to semi-continuous latex films [27,88]. In addition, by the increase of BuA content in the copolymer, the film abilities increase and Tg values decrease for copolymers produced by both process [27,85- 86,88].

Emulsion Polymerization:

Effects of Polymerization Variables on the Properties of Vinyl Acetate Based Emulsion Polymers 61

(PVOH) and polymerizable oligomeric N-methylol acrylamide (o-NMA). The VAc/BuA copolymer latexes obtained by o-NMA at different copolymer compositions were found to have lower viscosity, finer particle size, better latex stability and lower MWD and their films showed the higher Tg, better film forming behavior and better water resistance, compared to those synthesized by PVOH. Figure 3 shows the effect of the BuA content and the stabilizing system on the Tg of the VAc/BuA latex films [85]. They also compared the effects of two different initiator systems which consist of ammonium persulfate and potassium persulafte, on the properties of VAc/BuA copolymers synthesized in presence of o-NMA. It was seen that the particle size of copolymers varied by the increasing BuA content in the copolymer regardless of the type of initiator. Otherwise, for the all copolymer compositions, molecular weights (MWs) of the copolymers synthesized in the presence of potassium persulfate were found to be higher and the latex viscosities of them were lower, than those of VAc/BuA

copolymers synthesized in the presence of ammonium persulfate [83].

**Figure 3.** Changes in Tg with copolymer composition for VAc/BuA copolymer latexes obtained by o-

The seeded emulsion polymerization process can be applied for VAc/BuA comonomer system. Seeded reactions allow for the production of mono-dispersee latexes. Key factors in producing narrow PSD latexes are concentration of seed latex and ionic strength. The increasing of seed latex concentration (55% by weight) causes to the largest mono-dispersee

The emulsion copolymerization of VAc/BuA monomer system can be performed by other emulsion polymerization methods, mini-emulsion and micro-emulsion polymerizations. When the mini-emulsion copolymerization carries out with the 50/50 molar ratio of VAc/BuA in the presence of sodium hexadecyl sulfate emulsifier, hexadecane co-surfactant and ammonium persulfate initiator, the results of this polymerization conducted in a batch process are different from that of conventional batch polymerization of this monomer couple [94]. For the mini-emulsion polymerization the polymerization rate is slowed done,

NMA and PVOH [85]

particles [93].

The semi-continuous copolymerization of VAc/BuA monomer system can be carried out by applying different addition policy of copolymerization ingredients. In the copolymerization of VAc/BuA system having a certain monomer ratio, the monomer addition type directly affects the course of copolymerization. For seeded-semi-continuous copolymerizations in which a certain part of monomer present in the initial reactor charge as a remaining part in the feeding, the polymerization rate approaches a constant value depending on the monomer addition rate when the monomer-starved feed addition strategy is applied (for a neat monomer feed method). It increases with increasing monomer addition rate, and approaches the rate observed for batch polymerization when the feed rates exceed the maximum values for monomer –starved conditions. In the other hand, the polymerization rate is at maximum and independent upon the monomer feed rate when monomer-flooded condition is applied [87,89]. Furthermore, for the semi-continuous process of VAc/BuA, micro-phase separation in particle structure is revealed, and the feeding rate of comonomers influences the change in this particle morphology of copolymers. The faster feeding rate causes to greater separation while a multi-core-shell structure is formed with the slowest feeding [90]. The initiator addition policy also affects the polymerization rate, the instantaneous monomer conversion, the average PS and PSD, and the polymerization stability of the VAc/BuA semi-continuous emulsion systems. Increasing the amount of ammonium persulfate initiator in the initial reactor charge leads to increase the rate of polymerization and the conversion. But it is observed that this amount is increased above a certain value, destabilization occurs and the average PS increase [91-92].

The stabilizing system significantly affects many colloidal and film properties of the VAc/BuA emulsion copolymers. Berber and co-workers studied the semi-continuous emulsion copolymerization of this comonomer system in the presence of conventional nonionic emulsifiers and different protective colloids which were water-soluble polymer (PVOH) and polymerizable oligomeric N-methylol acrylamide (o-NMA). The VAc/BuA copolymer latexes obtained by o-NMA at different copolymer compositions were found to have lower viscosity, finer particle size, better latex stability and lower MWD and their films showed the higher Tg, better film forming behavior and better water resistance, compared to those synthesized by PVOH. Figure 3 shows the effect of the BuA content and the stabilizing system on the Tg of the VAc/BuA latex films [85]. They also compared the effects of two different initiator systems which consist of ammonium persulfate and potassium persulafte, on the properties of VAc/BuA copolymers synthesized in presence of o-NMA. It was seen that the particle size of copolymers varied by the increasing BuA content in the copolymer regardless of the type of initiator. Otherwise, for the all copolymer compositions, molecular weights (MWs) of the copolymers synthesized in the presence of potassium persulfate were found to be higher and the latex viscosities of them were lower, than those of VAc/BuA copolymers synthesized in the presence of ammonium persulfate [83].

60 Polymer Science

86,88].

effects hydrolysis and electrolyte resistance of the latexes [27,82]. The broader molecular weight distribution (MWD) with bimodal character is observed for semi-continuous copolymers. The MWD of batch copolymers are broad, but they are narrower and in unimodal character in comparison to those of semi-continuous copolymers. This results for both processes indicates the excessive branching reactions [27,82-85,87]. When the film properties of VAc/BuA copolymer latexes of various copolymer composition are examined, it is seen that the semi-continuous process provide better properties to copolymer films such as filming ability and film homogeneity (examined according to the Tg and surface analyzes) than the batch process [27,88]. The homogeneity influences hardness and adhesive properties of latexes as well as copolymer composition, and hardness decreases with increasing homogeneity [79]. The thermodynamic work of adhesion decreases with increasing BuA content for semi-continuous copolymer films [86]. In contrast, tensile properties of the batch copolymer films show a higher ultimate tensile strength, higher Young's modulus, and lower percent elongation to break compared to semi-continuous latex films [27,88]. In addition, by the increase of BuA content in the copolymer, the film abilities increase and Tg values decrease for copolymers produced by both process [27,85-

The semi-continuous copolymerization of VAc/BuA monomer system can be carried out by applying different addition policy of copolymerization ingredients. In the copolymerization of VAc/BuA system having a certain monomer ratio, the monomer addition type directly affects the course of copolymerization. For seeded-semi-continuous copolymerizations in which a certain part of monomer present in the initial reactor charge as a remaining part in the feeding, the polymerization rate approaches a constant value depending on the monomer addition rate when the monomer-starved feed addition strategy is applied (for a neat monomer feed method). It increases with increasing monomer addition rate, and approaches the rate observed for batch polymerization when the feed rates exceed the maximum values for monomer –starved conditions. In the other hand, the polymerization rate is at maximum and independent upon the monomer feed rate when monomer-flooded condition is applied [87,89]. Furthermore, for the semi-continuous process of VAc/BuA, micro-phase separation in particle structure is revealed, and the feeding rate of comonomers influences the change in this particle morphology of copolymers. The faster feeding rate causes to greater separation while a multi-core-shell structure is formed with the slowest feeding [90]. The initiator addition policy also affects the polymerization rate, the instantaneous monomer conversion, the average PS and PSD, and the polymerization stability of the VAc/BuA semi-continuous emulsion systems. Increasing the amount of ammonium persulfate initiator in the initial reactor charge leads to increase the rate of polymerization and the conversion. But it is observed that this amount is increased above a

certain value, destabilization occurs and the average PS increase [91-92].

The stabilizing system significantly affects many colloidal and film properties of the VAc/BuA emulsion copolymers. Berber and co-workers studied the semi-continuous emulsion copolymerization of this comonomer system in the presence of conventional nonionic emulsifiers and different protective colloids which were water-soluble polymer

**Figure 3.** Changes in Tg with copolymer composition for VAc/BuA copolymer latexes obtained by o-NMA and PVOH [85]

The seeded emulsion polymerization process can be applied for VAc/BuA comonomer system. Seeded reactions allow for the production of mono-dispersee latexes. Key factors in producing narrow PSD latexes are concentration of seed latex and ionic strength. The increasing of seed latex concentration (55% by weight) causes to the largest mono-dispersee particles [93].

The emulsion copolymerization of VAc/BuA monomer system can be performed by other emulsion polymerization methods, mini-emulsion and micro-emulsion polymerizations. When the mini-emulsion copolymerization carries out with the 50/50 molar ratio of VAc/BuA in the presence of sodium hexadecyl sulfate emulsifier, hexadecane co-surfactant and ammonium persulfate initiator, the results of this polymerization conducted in a batch process are different from that of conventional batch polymerization of this monomer couple [94]. For the mini-emulsion polymerization the polymerization rate is slowed done,

the final particle size is larger and the coagulation during the polymerization occurs, compared to the conventional batch process. There is also less mixing between the BuA-rich core and VAc-rich shell. The presence of co-surfactant makes significant effects to both of course of the copolymerization and the resulting latex and films [94].

Emulsion Polymerization:

Effects of Polymerization Variables on the Properties of Vinyl Acetate Based Emulsion Polymers 63

including hydroxylethyl cellulose (HEC) as protective colloid and sodium sulfosuccinate of 6 moles ethoxylated nonyl phenol as emulsifier compared to the VAc/DBM system. They also used n-butanol as chain transfer agent. The comonomer addition was applied in flooded conditions for a certain comonomer ratio, VAc/2-ethylhexyl maleate: 80/20 by volume). They investigated the effect of HEC on the particle number, conversion, and latex surface tension during the copolymerization. The oscillations occurred in these investigation parameters due to the flocculation and nucleation of new particles. The authors suggested that HEC splits its chain in the presence of the initiator, thus continuously stabilizing the new particles formed. In theVAc/2-ethylhexyl maleate copolymerization system, it was seen that the copolymerization rate and conversion decreased with the increasing agitation rate. The higher the agitation rate also affected the average PS of copolymers, and the smaller the PS found up to 600 rpm agitation rate. In addition, the presence of n-butanol in that reaction

system decreased the average particle diameter and cross-linked copolymer content.

the copolymer MW.

Wu and Schork also studied the copolymerization of VAc/DOM for different compositions of monomer mixture. They compared the conventional (macro-) and the mini-emulsion polymerization by applying both of batch and semi-continuous process [95]. In their study, a certain difference in PSs and particle numbers between macro-emulsion and miniemulsion feed semi-continuous operation is seen. The PS is smaller and the particle number is higher. The size decreases with a decrease in feed rate for both macro- and mini-emulsion polymerization. The PSs in semi-continuous operations are smaller than in batch miniemulsion polymerizations when the feed rate of monomer emulsion is sufficiently low. For batch copolymerizations of VAc and DOM, the rate of macro-emulsion polymerization is faster than that of mini-emulsion polymerization while the particle number increases with increasing conversion throughout the reaction for both macro- and mini-emulsion processes. Due to the extremely water-insoluble DOM monomer, a significant deviation in the composition of the VAc/DOM copolymer is observed. The most homogeneous compositions are obtained by mini-emulsion copolymerizations and the coagulation resistance of this emulsion polymerization system is better than that of macro-emulsion process, as well. For both of macro- and mini-emulsion polymerizations, the increasing concentration of DOM in the monomer mixture results in a reduction of the total polymerization rate and reduction of

Berber investigated the effects of some polymerization variables such as process type, initiator addition type, emulsifier type and its distribution between the initial reactor charge and feed, and feeding time on the monomer conversion, the latex stability and the average particle size for semi-continuous emulsion copolymerizations of VAc with DOM (VAc/DOM: 60/40, by weight) [99]. The emulsion copolymerizations were carried out in the presence of potassium persulfate as initiator and o-NMA as polymerizable co-stabilizer. A mixture of monomers, such as including VAc and DOM, should be added to reaction medium by the monomer emulsion feed method because of the large water-solubility differences between the two monomers. Thus, the selected emulsifier system should constitute "pre-emulsion" for monomer emulsion feed of the monomer couple. For the mixture of VAc and DOM monomers, anionic and non-ionic emulsifiers such as sodium

The emulsion copolymerizations of vinyl acetate with maleic acid diesters such as dibutyl maleate (DBM) and dioctyl maleate (DOM) are also possible. These diesters are easily copolymerized but can not homopolymerize. The main features of these monomer couples are: reactivity ratios (rVAc=0.171 and rDBM=0.046; rVAc=0.195 and rDOM=0.945) and water solubilities (25 g/L for VAc, 0.35 g/L for DBM and almost zero for DOM, at 20 oC) [95-96]. Because of the significantly different monomer properties between VAc and these maleic acid diesters, copolymer latexes having a wide range of properties can be obtained by varying the comonomer composition, thus influencing the glass transition temperature and minimum film forming temperature of the latexes. The use of these comonomers provides internal plastification to VAc polymers and they reduce the Tg value of them. The hardness, flexibility, and alkali, water and ultra-violet light resistance of their films can be improved. Furthermore, these diesters gain more stability to the copolymer latex by being strongly associated to the latex particles. It is then expected that the final properties of the copolymers will be enhanced and will not be altered during time due for instance to the migration of the plasticizer. The copolymers of VAc/Maleic acid diester are used for paints and adhesives.

Although these copolymers are industrially very useful, there are no more scientific researches about them. The earliest studies in the literature about the VAc/Maleic acid diester copolymers belong to Donescu and co-workers [57,97]. They investigated the semicontinuous emulsion polymerization of VAc and DBM (VAc/DBM: 60/40 by volume). They used PVOH, 20 moles ethoxylated cetyl alcohol and potassium persulfate as protective colloid, emulsifier and initiator respectively. The seeded-semi-continuous process was carried out by applying monomer emulsion feed method. The effects of emulsifier distribution between initial reactor charge and continuously introduced monomer, and agitation speed on the monomer conversion and copolymer structure were also investigated. They observed decrease in the polymerization rate with an increase of agitation speed. On the other hand, the transfer reactions were higher for the smaller speed. When the influence of the emulsifier distribution on conversion was examined, it was seen that the conversion increased and then decreased with the increasing initial reactor charge concentration of emulsifier. This behavior has been explained that the chain transfer effect of emulsifier is more pronounced over a certain emulsifier concentration. The emulsifier and DBM act as chain transfer agent in this type emulsion copolymerization of VAc/DBM [57]. In addition, Donescu and Fusulan copolymerized VAc with DBM using a semi-continuous process for different copolymer compositions. They also noticed a decrease in particle size with increasing DBM monomer. The retarding effect of DBM on the VAc polymerization was also determined [98]. In another study, Donescu and co-workers copolymerized VAc with another type of maleic acid diesters, 2-ethylhexyl maleate which is synonym for DOM, by semi-continuous emulsion polymerization [97]. They used a different stabilizing system including hydroxylethyl cellulose (HEC) as protective colloid and sodium sulfosuccinate of 6 moles ethoxylated nonyl phenol as emulsifier compared to the VAc/DBM system. They also used n-butanol as chain transfer agent. The comonomer addition was applied in flooded conditions for a certain comonomer ratio, VAc/2-ethylhexyl maleate: 80/20 by volume). They investigated the effect of HEC on the particle number, conversion, and latex surface tension during the copolymerization. The oscillations occurred in these investigation parameters due to the flocculation and nucleation of new particles. The authors suggested that HEC splits its chain in the presence of the initiator, thus continuously stabilizing the new particles formed. In theVAc/2-ethylhexyl maleate copolymerization system, it was seen that the copolymerization rate and conversion decreased with the increasing agitation rate. The higher the agitation rate also affected the average PS of copolymers, and the smaller the PS found up to 600 rpm agitation rate. In addition, the presence of n-butanol in that reaction system decreased the average particle diameter and cross-linked copolymer content.

62 Polymer Science

and adhesives.

the final particle size is larger and the coagulation during the polymerization occurs, compared to the conventional batch process. There is also less mixing between the BuA-rich core and VAc-rich shell. The presence of co-surfactant makes significant effects to both of

The emulsion copolymerizations of vinyl acetate with maleic acid diesters such as dibutyl maleate (DBM) and dioctyl maleate (DOM) are also possible. These diesters are easily copolymerized but can not homopolymerize. The main features of these monomer couples are: reactivity ratios (rVAc=0.171 and rDBM=0.046; rVAc=0.195 and rDOM=0.945) and water solubilities (25 g/L for VAc, 0.35 g/L for DBM and almost zero for DOM, at 20 oC) [95-96]. Because of the significantly different monomer properties between VAc and these maleic acid diesters, copolymer latexes having a wide range of properties can be obtained by varying the comonomer composition, thus influencing the glass transition temperature and minimum film forming temperature of the latexes. The use of these comonomers provides internal plastification to VAc polymers and they reduce the Tg value of them. The hardness, flexibility, and alkali, water and ultra-violet light resistance of their films can be improved. Furthermore, these diesters gain more stability to the copolymer latex by being strongly associated to the latex particles. It is then expected that the final properties of the copolymers will be enhanced and will not be altered during time due for instance to the migration of the plasticizer. The copolymers of VAc/Maleic acid diester are used for paints

Although these copolymers are industrially very useful, there are no more scientific researches about them. The earliest studies in the literature about the VAc/Maleic acid diester copolymers belong to Donescu and co-workers [57,97]. They investigated the semicontinuous emulsion polymerization of VAc and DBM (VAc/DBM: 60/40 by volume). They used PVOH, 20 moles ethoxylated cetyl alcohol and potassium persulfate as protective colloid, emulsifier and initiator respectively. The seeded-semi-continuous process was carried out by applying monomer emulsion feed method. The effects of emulsifier distribution between initial reactor charge and continuously introduced monomer, and agitation speed on the monomer conversion and copolymer structure were also investigated. They observed decrease in the polymerization rate with an increase of agitation speed. On the other hand, the transfer reactions were higher for the smaller speed. When the influence of the emulsifier distribution on conversion was examined, it was seen that the conversion increased and then decreased with the increasing initial reactor charge concentration of emulsifier. This behavior has been explained that the chain transfer effect of emulsifier is more pronounced over a certain emulsifier concentration. The emulsifier and DBM act as chain transfer agent in this type emulsion copolymerization of VAc/DBM [57]. In addition, Donescu and Fusulan copolymerized VAc with DBM using a semi-continuous process for different copolymer compositions. They also noticed a decrease in particle size with increasing DBM monomer. The retarding effect of DBM on the VAc polymerization was also determined [98]. In another study, Donescu and co-workers copolymerized VAc with another type of maleic acid diesters, 2-ethylhexyl maleate which is synonym for DOM, by semi-continuous emulsion polymerization [97]. They used a different stabilizing system

course of the copolymerization and the resulting latex and films [94].

Wu and Schork also studied the copolymerization of VAc/DOM for different compositions of monomer mixture. They compared the conventional (macro-) and the mini-emulsion polymerization by applying both of batch and semi-continuous process [95]. In their study, a certain difference in PSs and particle numbers between macro-emulsion and miniemulsion feed semi-continuous operation is seen. The PS is smaller and the particle number is higher. The size decreases with a decrease in feed rate for both macro- and mini-emulsion polymerization. The PSs in semi-continuous operations are smaller than in batch miniemulsion polymerizations when the feed rate of monomer emulsion is sufficiently low. For batch copolymerizations of VAc and DOM, the rate of macro-emulsion polymerization is faster than that of mini-emulsion polymerization while the particle number increases with increasing conversion throughout the reaction for both macro- and mini-emulsion processes. Due to the extremely water-insoluble DOM monomer, a significant deviation in the composition of the VAc/DOM copolymer is observed. The most homogeneous compositions are obtained by mini-emulsion copolymerizations and the coagulation resistance of this emulsion polymerization system is better than that of macro-emulsion process, as well. For both of macro- and mini-emulsion polymerizations, the increasing concentration of DOM in the monomer mixture results in a reduction of the total polymerization rate and reduction of the copolymer MW.

Berber investigated the effects of some polymerization variables such as process type, initiator addition type, emulsifier type and its distribution between the initial reactor charge and feed, and feeding time on the monomer conversion, the latex stability and the average particle size for semi-continuous emulsion copolymerizations of VAc with DOM (VAc/DOM: 60/40, by weight) [99]. The emulsion copolymerizations were carried out in the presence of potassium persulfate as initiator and o-NMA as polymerizable co-stabilizer. A mixture of monomers, such as including VAc and DOM, should be added to reaction medium by the monomer emulsion feed method because of the large water-solubility differences between the two monomers. Thus, the selected emulsifier system should constitute "pre-emulsion" for monomer emulsion feed of the monomer couple. For the mixture of VAc and DOM monomers, anionic and non-ionic emulsifiers such as sodium

dodecylbenzene sulfonate (Maranil A 25), dioctyl sodium sulfosuccinate (Disponil SUS 87), sodium lauryl ether sulphate (SLES), 30 and 10 moles ethoxylated nonyl phenoles (NP 30 and NP 10), and their combinations were used. The non-ionic emulsifiers system consisting of equal amounts of NP 30 and NP 10 which can form stable pre-emulsion and can produce stable copolymer latex was selected as suitable emulsifier system for VAc/DOM emulsion copolymerization (Table 1). The change of emulsifier concentration in the initial reactor charge (from 0% to 33%, by weight) affected the stability of polymerization and the average PS of copolymer latexes. The very high or the very low concentrations of emulsifier in the initial charge caused to polymerization instability and increase in average PS (Table 2).

Emulsion Polymerization:

82 145

86 160

95 221

Particle size (nm)

(%)

Effects of Polymerization Variables on the Properties of Vinyl Acetate Based Emulsion Polymers 65

as 5 portion during feeding

as drop wise during feeding

half of the total amount at beginning of the reaction

the remaining amount as drop wise during feeding

time

time

+

time

Initiator feed Conversion

Completion stage

70 oC, 30 min.

70 oC, 1 h.

80 oC, 1h.

**Table 3.** The effect of some polymerization variables on conversion and particle size of VAc/DOM latex

Vinyl versatate monomer (vinyl ester of versatic acid) is a commercial product of Shell Chemicals and called as VeoVA. It is a branched vinyl neodecanoate, and this branched vinyl ester (VeoVA 10) is copolymerized with VAc. The reactivity ratios of VAc and vinyl neodecanoate are respectively 0.99 and 0.92. The water solubilities are 25 g/L for VAc and 0.1 g/L for vinyl neodecanoate at 20 oC. The glass transition temperatures are 32 oC for PVAc and –3 oC for polyVeoVa. VeoVA can act as internal plasticizer in VAc emulsion copolymers. The most distinguishing feature of these branched vinyl esters is their resistance to hydrolysis, both as monomers and in polymers. Polymerization of branched vinyl esters with VAc results in polymers whose hydrolytic stability improves with increasing concentrations of branched vinyl ester. Higher molar mass vinyl branched esters offer excellent hydrophobic properties. These esters are strongly resistant to saponification, water absorption and UV degredation. The properties of VAc polymer such as water and alkali resistance and exterior durability improve with these esters. These all advantages make the VAc/branched vinyl ester copolymers more suitable for applications. They are used in architectural paints, interior and exterior applications, and general markets, Typically, about 15-30% VeoVa-10 is used to optimize the cost-performance properties of VAc polymers. Interior latexes tend to contain 15-20% monomer. Exterior latexes usually contain 20-30% of the branched monomer [15,30]. The high solids emulsion copolymerization of VAc and VeoVA 10 can be carried out in a continuous industrial reactors, continuous loop reactor and continuous stirred tank reactor (CSTR). When the heat

Monomer content in initial reactor charge (%, w/w)

10

Seeding stage

30 min. at 65 oC + 30 min. at 70 oC Feeding stage

70 oC, 2.5 h.

70 oC, 3 h.

70 oC, 5 h.

**Table 1.** The effects of emulsifier type on the stability of pre-emulsion and resulting latex for VAc/DOM system

**Table 2.** The effects of emulsifier concentration in initial reactor charge on the stability and the particle size of latex for VAc/DOM system

In addition, the presence of seeding stage in the semi-continuous process (by 10 wt % monomer), the increasing of the feeding time and better control of the initiator feed increased the monomer conversion, the average particle size, and the stabilities of the polymerization and latex of VAc/DOM monomer system. The effect of these reaction variables on the conversion and the particle size of the VAC/DOM latex are given in Table 3 [99].

system

[99].

Emulsifier concentration in initial reactor charge (%, w/w)

size of latex for VAc/DOM system

dodecylbenzene sulfonate (Maranil A 25), dioctyl sodium sulfosuccinate (Disponil SUS 87), sodium lauryl ether sulphate (SLES), 30 and 10 moles ethoxylated nonyl phenoles (NP 30 and NP 10), and their combinations were used. The non-ionic emulsifiers system consisting of equal amounts of NP 30 and NP 10 which can form stable pre-emulsion and can produce stable copolymer latex was selected as suitable emulsifier system for VAc/DOM emulsion copolymerization (Table 1). The change of emulsifier concentration in the initial reactor charge (from 0% to 33%, by weight) affected the stability of polymerization and the average PS of copolymer latexes. The very high or the very low concentrations of emulsifier in the initial charge caused to polymerization instability and increase in average PS (Table 2).

Emulsifiers Stable Pre-emulsion Stable Latex Maranil A 25 - - Disponil SUS 87 - - SLES - - NP 30 - - NP 10 - - % 70 SLES + % 30 NP 10 - % 30 NP 30 + % 70 NP 10 - % 50 NP 30 + % 50 NP 10

**Table 1.** The effects of emulsifier type on the stability of pre-emulsion and resulting latex for VAc/DOM

33 Creaming and incrustation on the latex surface

25 Partially incrustation on the latex

0 Coagulation and incrustation on the latex surface

**Table 2.** The effects of emulsifier concentration in initial reactor charge on the stability and the particle

In addition, the presence of seeding stage in the semi-continuous process (by 10 wt % monomer), the increasing of the feeding time and better control of the initiator feed increased the monomer conversion, the average particle size, and the stabilities of the polymerization and latex of VAc/DOM monomer system. The effect of these reaction variables on the conversion and the particle size of the VAC/DOM latex are given in Table 3

surface

Appearance of latex Particle size (nm)

284

221

482

**Table 3.** The effect of some polymerization variables on conversion and particle size of VAc/DOM latex

Vinyl versatate monomer (vinyl ester of versatic acid) is a commercial product of Shell Chemicals and called as VeoVA. It is a branched vinyl neodecanoate, and this branched vinyl ester (VeoVA 10) is copolymerized with VAc. The reactivity ratios of VAc and vinyl neodecanoate are respectively 0.99 and 0.92. The water solubilities are 25 g/L for VAc and 0.1 g/L for vinyl neodecanoate at 20 oC. The glass transition temperatures are 32 oC for PVAc and –3 oC for polyVeoVa. VeoVA can act as internal plasticizer in VAc emulsion copolymers. The most distinguishing feature of these branched vinyl esters is their resistance to hydrolysis, both as monomers and in polymers. Polymerization of branched vinyl esters with VAc results in polymers whose hydrolytic stability improves with increasing concentrations of branched vinyl ester. Higher molar mass vinyl branched esters offer excellent hydrophobic properties. These esters are strongly resistant to saponification, water absorption and UV degredation. The properties of VAc polymer such as water and alkali resistance and exterior durability improve with these esters. These all advantages make the VAc/branched vinyl ester copolymers more suitable for applications. They are used in architectural paints, interior and exterior applications, and general markets, Typically, about 15-30% VeoVa-10 is used to optimize the cost-performance properties of VAc polymers. Interior latexes tend to contain 15-20% monomer. Exterior latexes usually contain 20-30% of the branched monomer [15,30]. The high solids emulsion copolymerization of VAc and VeoVA 10 can be carried out in a continuous industrial reactors, continuous loop reactor and continuous stirred tank reactor (CSTR). When the heat generation rate is high a thermal runaway occurred in the CSTR reactor, whereas the loop reactor is easily controlled [100].

Emulsion Polymerization:

Effects of Polymerization Variables on the Properties of Vinyl Acetate Based Emulsion Polymers 67

continuous, continuous and seeded, and their application types. Secondly, the emulsion polymerization of vinyl acetate was given. The characteristic feature of vinyl acetate monomer, its emulsion polymerization conditions, and the main properties of its homopolymer latex were summarized. Finally, the emulsion copolymerizations of vinyl acetate with other monomers having specific features and industrially importance were discussed briefly. The effects of the copolymerization variables and the components on the course of emulsion polymerization and the properties of the resulting copolymers were

[1] Hoffman F and Delbrück K (1909) German Patent. 250,690 (to Farbenfabriken Bayer

[2] Hoffman F and Delbrück K (1912) German Patent. 254,672 (to Farbenfabriken Bayer

[3] Hoffman F and Delbrück K (1912) German Patent. 255,129 (to Farbenfabriken Bayer

[6] Starck W and Freudenberg H (1940) U.S. Patent. 2,227,163 (to I.G Farbenindustrie A.G). [7] B.I.O.S (British Intelligence Objectives Subcommision) (1947) Manufacture of Vinyl

[8] US FIAT (Field Intelligence Agency Technical) (1947) Polymerization of Vinyl Acetate.

[9] B.I.O.S (British Intelligence Objectives Subcommision) (1954) The German Plastic Industry During the Period 1939-1945. Surveys Report 34. London: H.M.S.O. [10] Bovey F.A, Kolthoff I.M, Medalia, A.I, Meehan, E.J (1965) Emulsion Polymerization.

[11] Blackley D.C (1975) Emulsion Polymerization, Theory and Practice. London: Applied

[12] Eliseeva V.I, Ivanchev S.S, Kuchanov S.I, Lebedev A.V (1981). Emulsion Polymerization and Its Applications in Industry. New York: Plenum Publishing Corporation.

[14] Fitch M.R (1997) Polymer Colloids: A Comprehensive Introduction. USA: Academic

[15] Lovell P.A, El-Aasser M.S (1997) Emulsion Polymerization and Emulsion Polymers.

[4] Dinsmore R.P (1929) U.S. Patent. 1,732,975 (to Goodyear Tire & Rubber Co.). [5] Luther M and Hück C (1932) U.S. Patent. 1,864,078 (to I.G Farbenindustrie A.G).

Acetate Polymers and Derivatives. Final Report 744. London: H.M.S.O.

High Polymer Series Vol. IX. New York: Interscience Publishers Inc.

[13] Piirma I (1982) Emulsion Polymerization. New York:Academic Press.

Final Report 1102. London: H.M.S.O.

Science Publishers.

England: Wiley.

Press.

explained, which was supported by the literature results.

*Department of Chemistry, Yildiz Technical University, Istanbul, Turkey*

**Author details**

Hale Berber Yamak

**6. References**

A.G).

A.G).

A.G).